Composites are used extensively in engineering applications. A constant concern is the effect of foreign object impacts ...

Author:
Serge Abrate

This content was uploaded by our users and we assume good faith they have the permission to share this book. If you own the copyright to this book and it is wrongfully on our website, we offer a simple DMCA procedure to remove your content from our site. Start by pressing the button below!

Composites are used extensively in engineering applications. A constant concern is the effect of foreign object impacts on composite structures because significant damage can occur and yet be undetectable by visual inspection. Such impacts can range from the most ordinary at low velocity - a tool dropped on a product - to the hypervelocity impact of space debris on a spacecraft. This book brings together the latest developments in this important new research area. It explains how damage develops during impact, the effect of impact-induced damage on the mechanical behavior of structures, and methods of damage prediction and detection. Numerous examples are included to illustrate these topics. Written for graduate students, as well as for researchers and practicing engineers working with composite materials, this book presents state-of-the-art knowledge on impact dynamics, yet requires only basic understanding of the mechanics of composite materials.

IMPACT ON COMPOSITE STRUCTURES

IMPACT ON COMPOSITE STRUCTURES SERGE ABRATE Southern Illinois University at Carbondale

CAMBRIDGE UNIVERSITY PRESS

CAMBRIDGE UNIVERSITY PRESS Cambridge, New York, Melbourne, Madrid, Cape Town, Singapore, Sao Paulo Cambridge University Press The Edinburgh Building, Cambridge CB2 2RU, UK Published in the United States of America by Cambridge University Press, New York www.cambridge. org Information on this title: www.cambridge.org/9780521473897 © Cambridge University Press 1998 This book is in copyright. Subject to statutory exception and to the provisions of relevant collective licensing agreements, no reproduction of any part may take place without the written permission of Cambridge University Press. First published 1998 This digitally printed first paperback version 2005 A catalogue recordfor this publication is available from the British Library Library of Congress Cataloguing in Publication data Abrate, Serge, 1953Impact on composite structures / Serge Abrate. p. cm. Includes bibliographical references and index. ISBN 0-521-47389-6 (he) 1. Composite materials - Impact testing. 2. Composite materials - Mechanical properties. I. Title. TA418.9.C6A25 1998 624.1'89-dc21 97-16551 CIP ISBN-13 978-0-521-47389-7 hardback ISBN-10 0-521-47389-6 hardback ISBN-13 978-0-521-01832-6 paperback ISBN-10 0-521-01832-3 paperback

Contents

Preface 1 Introduction 2 Contact Laws 2.1 Introduction 2.2 Contact between Two Isotropic Elastic Solids 2.3 Indentation of Beams 2.4 Indentation of Plates 2.5 Indentation of a Laminate 2.6 Elastoplastic Models 2.7 Conclusion 2.8 Exercise Problems 3 Impact Dynamics 3.1 Introduction 3.2 Beam Theories 3.2.1 Bending of a Beam by a Uniform Load 3.2.2 Higher-Order Beam Theory 3.2.3 Timoshenko Beam Theory 3.2.4 Bernoulli-Euler Beam Theory 3.2.5 Static Loading on Beams 3.2.6 Recovery of Accurate Stresses from Beam Models 3.2.7 Harmonic Wave Propagation 3.2.8 Free Vibrations of Beams 3.2.9 Effect of Geometrical Nonlinearities 3.2.10 Summary 3.2.11 Exercise Problems 3.3 Plate Theories 3.3.1 First-Order Shear Deformation Theory 3.3.2 Classical Plate Theory (CPT)

ix 1 6 6 7 9 13 15 19 24 24 26 26 27 27 29 31 32 32 35 36 39 44 46 47 48 48 54

vi

Contents

3.3.3 Higher-Order Plate Theory (HOPT) 3.3.4 Static Deflections of Plates 3.3.5 Harmonic Wave Propagation 3.3.6 Free Vibrations of Plates 3.3.7 Transient Response of a Plate 3.3.8 Variational Models 3.3.9 Effect of Boundary Conditions 3.3.10 Summary 3.3.11 Exercise Problems 3.4 Impact Models 3.4.1 Spring-Mass Models 3.4.2 Energy Balance Models 3.4.3 Response of Bernoulli-Euler Beam to Impact by a Mass 3.4.4 Impact on a Simply Supported Plate (Classical Plate Theory) 3.4.5 Impact on a Simply Supported Plate (SDPT) 3.4.6 Approximate Solution for Wave-Controlled Impacts 3.4.7 Summary 3.4.8 Exercise Problems 3.5 Theory of Shells 3.5.1 Equations of Motion 3.5.2 Simply Supported Panels 3.5.3 Exercise Problems 3.6 Scaling 4 Low-Velocity Impact Damage 4.1 Impact Tests 4.2 Failure Modes in Low-Velocity Impact Damage 4.2.1 Morphology of Low-Velocity Impact Damage 4.2.2 Damage Development 4.2.3 Qualitative Models for Predicting Delamination Patterns 4.3 Experimental Methods for Damage Assessment 4.3.1 Nondestructive Techniques 4.3.2 Destructive Techniques 4.3.3 Observation of Damage Development during Impact 4.4 Parameters Affecting Impact Damage 4.4.1 Material Properties 4.4.2 Target Stiffness 4.4.3 Projectile Characteristics

55 59 63 70 71 75 79 82 82 83 83 86 89 96 99 113 126 127 128 128 131 132 132 135 136 140 140 144 145 148 148 150 151 151 152 154 154

Contents

5

6

7

8

4.4.4 Layup and Stitching 4.4.5 Preload 4.4.6 Environmental Conditions 4.5 Summary 4.6 Review Questions Damage Prediction 5.1 Introduction 5.2 Damage in Thick Laminates 5.3 Damage in Thin Laminates 5.4 Damage Initiation 5.5 Propagation of Delaminations during Impact 5.6 Conclusion 5.7 Exercises Residual Properties 6.1 Introduction 6.2 Compressive Strength 6.2.1 Test Procedures 6.2.2 Experimental Results 6.2.3 Prediction of Residual Compressive Strength 6.3 Buckling 6.3.1 Thin-Film Delaminations 6.3.2 Delaminated Beam-Plates 6.3.3 Buckling of Beam-Plates with Multiple Delaminations 6.3.4 Buckling of Delaminated Plates 6.4 Residual Tensile Strength 6.4.1 Experimental Results 6.4.2 Prediction of Residual Tensile Strength 6.5 Residual Flexural Strength 6.6 Fatigue 6.7 Effect of Impact Damage on Structural Dynamics Behavior 6.8 Exercise Problems Ballistic Impact 7.1 Introduction 7.2 Experimental Technique s 7.3 Ballistic Limit and Residual Velocity of the Projectile 7.4 Failure Modes 7.5 Prediction of Ballistic Limit 7.6 Ceramic-Composite Armor Repairs 8.1 Introduction

vii 157 158 158 158 159 161 161 162 163 165 168 170 171 172 172 172 173 177 185 186 189 190 193 195 198 199 201 205 206 209 213 215 215 216 217 219 220 224 228 228

viii

Contents

8.2 Mechanically Fastened Patches 8.3 Adhesive Bonded Joints 8.3.1 Peel and Shear Stresses in a Double-Lap Joint 8.3.2 Bonded Metal Patch Repair 8.3.3 Bonded Composite Repair 8.3.4 Staggered Bonded Repair 8.3.5 Repair of Composite Sandwich Structures 8.3.6 Resin Injection 8.4 Repair of Thermoplastic Composites 9 Impact on Sandwich Structures 9.1 Introduction 9.2 Contact Laws 9.2.1 Compressive Behavior of Core Materials 9.2.2 Contact between a Sandwich Beam and a Cylindrical Indentor 9.2.3 Contact between a Sandwich Plate and a Spherical Indentor 9.3 Impact Dynamics 9.4 Impact Damage 9.4.1 Failure Modes 9.4.2 Governing Parameters 9.4.3 Improved Sandwich Construction 9.4.4 High-Velocity Impacts 9.5 Residual Properties References Index

230 231 232 235 236 236 237 237 238 240 240 240 241 245 247 248 249 249 251 254 255 255 258 287

Preface

As composite materials are used more extensively, a constant source of concern is the effect of foreign objects impacts. Such impacts can reasonably be expected during the life of the structure and can result in internal damage that is often difficult to detect and can cause severe reductions in the strength and stability of the structure. This concern provided the motivation for intense research resulting in hundreds of journal and conference articles. Important advances have been made, and many aspects of the problem have been investigated. One would need to study a voluminous literature in order to get an appreciation for this new research area. After writing three comprehensive literature reviews on the topic of impact on composite materials, I felt that there was a need to present this material in book form. The study of impact on composite structures involves many different topics, including contact mechanics, structural dynamics, strength, stability, fatigue, damage mechanics, and micromechanics. Impacts are simple events with many complicated effects, and what appears as a logical conclusion in one situation seems to be completely reversed in another. This variety and complexity have kept me interested in this area for several years, and I hope to communicate that to the readers. This book attempts to present this new body of knowledge in a unified, detailed, and comprehensive manner. It assumes only a basic knowledge of solid mechanics and the mechanics of composite materials and can be used as a text for a graduate-level course or for self-study. Exercise problems are proposed in order to challenge the user's understanding of the material. It is hoped that, after each section, the reader will gain an appreciation of the problems being addressed and the methods available and will be able to implement some of these methods. For example, after Chapter 3, "Impact Dynamics," the reader should understand what is involved in the selection of a mathematical model for predicting the contact force history and should be able to implement what appears to be the logical choice for the particular problem being considered. IX

x

Preface

Researchers and practitioners in industry would appreciate this comprehensive presentation of the state of the art in this area and use this book as a reference. A long list of references is included for those interested in more details. Current knowledge in certain areas has reached a certain level of maturity. For example, there is a general agreement on how to model the local indentation of a composite plate by smooth indentors. In other areas, current methods are not completely satisfactory, particularly in the areas of damage prediction and the prediction of the residual properties of impact-damaged composites. The book covers both low-velocity and ballistic impacts. Hypervelocity impacts encountered when spacecraft are hit by meteorites or space debris are in a different class, where impact velocities are measured in km/s. Too few studies dealing with this type of impacts on composite structures can be found, so this aspect of the problem was omitted. Recently, a new area of research dealing with smart materials and smart structures has developed, and one of the objectives has been to use distributed sensors and actuators to monitor the health of the structure. Several attempts were made to determine if and where an impact occurred or to determine the location and size of impact damage. This type of study is beyond the scope of this book, because it would require discussing the modeling of such sensors and actuators, control methods, and identification procedures. However, the methods for modeling the impact dynamics and for modeling the behavior of damaged structures discussed in this book will be very useful for modeling such smart structures. Upon reading this book, it will be obvious that I am indebted to the numerous investigators who have contributed to the development of this body of knowledge. I have made an effort to include every significant development and to acknowledge the source. A book is usually a reflection of the author's choices regarding what needed to be included and what could be omitted. A balance must be struck between the desire to be clear and comprehensive and the risk of overburdening the reader. In this case, almost every chapter could have been expanded to full book length, making it sometimes difficult to choose. However, I hope readers will gain a sufficient understanding of each aspect of the problem that they will be able to pursue its study on their own. The extensive list of references and the several available literature surveys should be helpful in this regard. Finally, I would like to thank my editor, Florence Padgett, for being so supportive of me in this endeavor. My wife Jayne and my sons Denis and Marc deserve thanks for allowing me to devote much of my free time to this project. Special thanks to my parents, who encouraged me to pursue my dreams and helped me get the best education. I wish my father were still with us to see this book completed. He would have been very proud.

1 Introduction

During the life of a structure, impacts by foreign objects can be expected to occur during manufacturing, service, and maintenance operations. An example of in-service impact occurs during aircraft takeoffs and landings, when stones -and other small debris from the runway are propelled at high velocities by the tires. During the manufacturing process or during maintenance, tools can be dropped on the structure. In this case, impact velocities are small but the mass of the projectile is larger. Laminated composite structures are more susceptible to impact damage than a similar metallic structure. In composite structures, impacts create internal damage that often cannot be detected by visual inspection. This internal damage can cause severe reductions in strength and can grow under load. Therefore, the effects of foreign object impacts on composite structures must be understood, and proper measures should be taken in the design process to account for these expected events. Concerns about the effect of impacts on the performance of composite structures have been a factor in limiting the use of composite materials. For these reasons, the problem of impact has received considerable attention in the literature. The objective with this book is to present a comprehensive view of current knowledge on this very important topic. A first step in gaining some understanding of the problem is to develop mathematical models for predicting the force applied by the projectile on the structure during impact. In order to predict this contact force history, the model should account for the motion of the structure, the motion of the projectile, and the local deformations in the contact zone. A detailed description of the contact between the impactor and the structure during impact would be difficult to obtain and is not required as part of the impact dynamics analysis. Instead, what is needed is a contact law relating the contact force to the indentation, which is defined as the motion of the projectile relative to that of the target. With the material systems commonly used, strain rate effects are negligible such 1

2

1 Introduction

that static and dynamic contact laws are identical, and so statically determined contact laws can be used in the dynamics analysis. Many investigators analyzed the loading phase of the indentation process and predicted the contact law for beams and plates with various boundary conditions and several indentor shapes. The indentation process introduces damage and permanent deformations in the contact zone; as a result, the unloading curve differs from the loading curve. In many cases, multiple impacts occur and the reloading curve is again different. While some simple analyses of the unloading and reloading phases have been presented, a complete and accurate characterization of the contact law for a particular target-indentor combination can only be obtained experimentally. A set of equations are commonly used to describe the contact behavior between solid laminates and smooth indentors, with a small number of constants to be determined from experiments. Contact problems are discussed in Chapter 2. An important aspect of a model for predicting the impact dynamics is to accurately describe the dynamic behavior of the target. For some simple cases, the motion of the structure can be modeled by a simple spring-mass system or by assuming a quasi-static behavior and considering the balance of energy in the system. But in general, more sophisticated beam, plate, or shell theories are required to model the structure. Two- and three-dimensional elasticity models are also employed. For each particular case, a choice must be made between a number of theories developed to account for complicating factors such as transverse shear deformation and rotary inertia. In addition, one must select to use variational approximation methods or finite element methods if exact solutions are not available for the case at hand. In Chapter 3, several structural theories are presented and their accuracies are discussed, particularly in regard to the impact problem. Several examples of impact dynamics analyses are presented for impacts on beams, plates, and shells. Often tests cannot be performed on full scale prototypes, so small specimens must be used. In other cases, tests or analyses have been performed on two specimens of different sizes. Methods developed to scale results obtained from a small-scale model to a full-size prototype are discussed in Chapter 3. Different test apparatus are used to simulate various types of impact. Dropweight testers are used to simulate low-velocity impacts typical of the tool-drop problem, in which a large object falls onto the structure with low velocity. Airgun systems, in which a small projectile is propelled at high speeds, are used to simulate the type of impacts encountered during aircraft takeoffs and landings. Testing conditions should replicate the actual impacts the structure is designed to withstand, and so the choice of the proper test apparatus is important. Descriptions of several common types of impact testers are given in Chapter 4, where damage development, the morphology of impact damage,

1 Introduction

3

and experimental techniques for damage detection are also described. Impact damage consists of delaminations, matrix cracking, and fiber failure. Extensive experimental investigations have revealed definite patterns for the shape of the damage and its initiation and growth. It is generally accepted that during low-velocity impacts, damage is initiated by matrix cracks which create delaminations at interfaces between plies with different fiber orientations. For stiff structures, matrix cracks start on the impacted face of the specimen due to high contact stresses. Damage propagates downward by a succession of intra-ply cracks and interface delaminations to give what is called a pine tree pattern. For thin specimens, bending stresses cause matrix cracking in the lowest ply, and damage progresses from the nonimpacted face up toward the projectile giving a reverse pine tree appearance. Many studies demonstrated that no delaminations are induced at the interface between plies with the same fiber orientation. The delaminated area at an interface depends on the fiber orientations in the plies adjacent to that interface. Of the large number of experimental methods that have been developed for damage assessment, some result in the complete destruction of the specimen and others are nondestructive, but most methods are used to determine the state of damage after impact. A few methods can be used to monitor the development of damage during impact. Once the failure modes involved are known and methods to assess damage are available, the next task is to determine what the governing parameters are. The properties of the matrix, the reinforcing fibers, and the fiber-matrix interfaces affect impact resistance in several ways, along with effects of layup, thickness, size, boundary conditions, and the shape, mass, and velocity of the projectile. Techniques for improving both impact resistance and impact tolerance will also be discussed. The prediction of impact damage is a difficult task for which complete success may not be possible and is probably not necessary. A large number of matrix cracks and delaminations are created in the impact zone, and the introduction of each new crack creates a redistribution of stresses. Thus it is not realistic to attempt to track every detail of damage development during the dynamic analysis of the impact event. Some purely qualitative models explain the orientation and size of delaminations at the various interfaces through the thickness of the laminate. Other models predict the onset of delaminations by predicting the appearance of the first matrix crack. Models for estimating the final state of delaminations are available. Chapter 5 deals with models for predicting impact damage. Impact-induced delaminations result in drastic reductions in strength, stiffness, and stability of the laminate, which explains why impact is of such concern to the designers and users of composite structures and why such effort has been directed at understanding the problem. Reductions are particularly significant

4

1 Introduction

in compression, where the effect of delaminations is more readily visible. The extent of these reductions has been characterized experimentally, and several mathematical models are used to predict the residual strength, as discussed in Chapter 6. Chapter 7 deals with high-velocity impacts. Sometimes the expression "highvelocity impact" refers to impacts resulting in complete perforation of the target. However, it must be recognized that complete perforation can be achieved both under low-velocity impacts when overall deflections of the target are taking place and under high-velocity impacts when the deformations of the target are localized in a small region near the point of impact. Here, high-velocity impacts are defined so that the ratio between impact velocity and the velocity of compressive waves propagating through the thickness is larger than the maximum strain to failure in that direction. This implies that damage is introduced during the first few travels of the compressive wave through the thickness when overall plate motion is not yet established. The ballistic limit is defined as the initial velocity of the projectile that results in complete penetration of the target with zero residual velocity. For impact velocities above the ballistic limit, the residual velocity of the projectile is also of interest. General trends for ballistic impacts (including the effect of several important parameters) are known from experimental results, and models for predicting the ballistic limit are available. Another area to be discussed in this chapter is the design of composite armor, which usually involves using one layer of ceramic material to blunt or fragment the projectile and another layer of composite material to absorb the residual kinetic energy. Many repair procedures for composite structures with impact damage have been reported. In selecting a particular repair technique, several factors must be considered, including the severity of the damage, the loads to be sustained, and the equipment available at the location where the repair procedure will be performed. In some cases, a successful repair cannot be made and the part must be replaced. In other cases, only cosmetic repairs are needed. In yet other cases, either bolted repairs or bonded repairs are needed. Proper design of the repair patch, machining, surface preparation, prefabrication of patches, and bonding are important phases of a successful repair procedure. The basic problems and most promising approaches are reported in Chapter 8. In many applications, sandwich structures with laminated facings are used because of the well-known advantages of this type of construction. The facings are loaded primarily in tension or compression to resist bending while the core resists the shear stresses. As a result, sandwich structures achieve a great bending rigidity, but in the transverse direction the rigidity remains low. A low rigidity in the transverse direction results in a low contact stiffness and

1 Introduction

5

lower contact forces during impact. Contact laws for sandwich structures are completely different from those of monolithic laminates and are dominated by the deformation of the core. Usually cores are made out of honeycomb materials, foam, or balsa wood. All these materials are considered to be part of the family of cellular materials and have a similar stress-strain behavior when loaded in compression in the transverse direction. The choice of a particular material is based on considerations of performance, weight, and cost. Models for predicting the behavior of a sandwich panel under a smooth indentor are discussed in Chapter 9. Impact creates damage to the facings, the core, and the core-facing interfaces. The evolution of damage with impact energy and its effects on the residual properties of sandwich panels are also discussed in that chapter.

2 Contact Laws

2.1 Introduction Local deformations in the contact region must be accounted for in the analysis in order to accurately predict the contact force history. The indentation, defined as the difference between the displacement of the projectile and that of the back face of the laminate, can be of the same order as or larger than the overall displacement of the laminate. One could consider the projectile and the structure as two solids in contact and then analyze the impact problem as a dynamic contact problem. However, this approach is computationally expensive and cannot describe the effect of permanent deformation and local damage on the unloading process. The unloading part of the indentation process can be modeled only using experimentally determined contact laws. To predict the contact force history and the overall deformation of the target, a detailed model of the contact region is not necessary. A simple relationship between the contact force and the indentation, called the contact law, has been used by Timoshenko (1913) to study the impact of a beam by a steel sphere. This approach has been used extensively since then and is commonly used for the analysis of impact on composite materials. Although the impact event is a highly dynamic event in which many vibration modes of the target are excited, statically determined contact laws can be used in the impact dynamics analysis of low-velocity impacts because strain rate and wave propagation effects are negligible with commonly used material systems. Hunter (1957) calculated the energy lost by elastic waves during the impact of a sphere on an elastic half-space. The ratio between the energy lost in the half-space and the initial kinetic energy of the sphere is given by V rV5 . 1.04 ( (2.1) Therefore, the energy loss is negligible as long as the initial velocity of the

22 Contact between Two Isotropic Elastic Solids

1

sphere, V, is small compared with c = (E/p)1^2, the phase velocity of compressive elastic waves in the solid. In many cases, the contact area is small and the behavior is similar to that observed during the indentation of a half-space. The indentation is independent of the overall deflection of the structure. When the contact area becomes large, the overall deflection of the structure affects the pressure distribution under the indentor; this interaction must be accounted for accurately. This chapter presents the basic results from contact mechanics needed to model the indentation of composite materials during the impact by a foreign object. The objective of such models is the accurate prediction of the contact force history and the overall response of the structure. 2.2 Contact between Two Isotropic Elastic Solids Detailed accounts of the study of contact between two smooth elastic solid pioneered by Hertz are given in several books (Barber 1992, Gladwell 1980, Johnson 1985, Timoshenko and Goodier 1970). Essential results from Hertz theory of contact as given here without derivation. For two isotropic bodies of revolution (Fig. 2.1), contact occurs in a circular zone of radius a in which the normal pressure p varies as

where po is the maximum contact pressure at the center of the contact zone and r is the radial position of an arbitrary point in the contact zone (Fig. 2.2). Defining the parameters R and E as

Figure 2.1. Two bodies of revolution for Hertzian analysis of contact.

2 Contact Laws

Figure 2.2. Pressure distribution in the contact zone.

where R\ and R2 are the radii of curvature of the two bodies. The Young moduli and Poisson's ratios of the two bodies are E\,v\, and E2, V2, respectively. Without loss of generality, the subscript 1 is taken to denote properties of the indentor and subscript 2 identifies properties of the target. The radius of the contact zone a, the relative displacement a, and the maximum contact pressure are given by a=

31

a3 ~R P0 =

(2.5)

—

' 4E =

( 9P2 \ ] \16RE2)

3P

2 i /6/>£2\ \

2*a* ~ V

(2.6) (2.7)

The force indentation law is expressed as P =

(2.8)

where P is the contact force, a is the indentation, and the contact stiffness k is given by k — —F /? 2"

o Q\

Equation (2.8) is usually referred to as Hertz contact law or the Hertzian law of contact and is found to apply for a wide range of cases, even if all the assumptions made in the derivation of the theory are not satisfied. For example, (2.8) also applies for laminated composites, even though these are not homogeneous and isotropic materials. With composite materials, permanent deformations are introduced in the contact zone for relatively low force levels, but the material is assumed to remain linear elastic in the analysis. Matrix cracks, fiber fracture, and interply delaminations can be introduced in the contact zone, but overall the contact law follows (2.8).

2.3 Indentation of Beams

9

The experimental determination of the contact law usually involves the use of a displacement sensor which directly measures the displacement of the indentor relative to the back face of the specimen. The plot of the applied force versus the indentation measured in this way follows the general form given by (2.8). Least-squares fits of the experimental data usually show that the exponent of a in that equation is close to | , and k is close to the value given by (2.9). Some investigators present plots of the contact force versus the displacement of the indentor that show a significant discontinuity when delaminations are introduced. The displacement of the indentor is the sum of the indentation and the deflection of the structure. The observed discontinuity corresponds to the reduction in the apparent stiffness of the structure caused by the introduction of delaminations.

2.3 Indentation of Beams During the indentation of beams, local deformations are superposed onto the overall deflection of the beam. When the beam deflections are small, the interaction between the local indentation and the overall deflection of the beam is negligible. Therefore, the indentation law and the pressure distribution in the contact zone are the same as for the indentation of a half-space. However, for flexible beams under large indentors, the beam may wrap around the indentor, leading to significant changes in the normal pressure distribution. First, consider the bending of a Bernoulli-Euler beam and neglect local deformations. This simple analysis will provide some understanding of the physical behavior of a beam loaded by a large indentor. From the free body diagram of an infinitesimal beam element (Fig. 2.3), the equilibrium equations for a planar beam are + V=0, (2.10) +p = 0, ^ dx dx where V is the shear force, M is the bending moment, and p is the applied force per unit length. With the Bernoulli-Euler beam theory, plane sections are assumed to remain planar and perpendicular to the neutral axis of the beam.

M

V Figure 2.3. Free body diagram of beam element.

10

2 Contact Laws

Figure 2.4. Simply supported beam with concentrated force applied in center. The axial displacements are then related to the transverse displacement by «(,,,) = -z*^>. dx

(2.11)

and the axial strain is d2w TTdx2 The bending moment is related to the transverse displacement by M = -

oxxzdA = JA

JA

(2-12)

EexxzdA JA

"2»

--*-

a,3,

The bending moment distribution in a simply supported beam of length L subjected to a concentrated force applied in the center (Fig. 2.4) is given by

for x > 0. The curvature of the beam is given by the second derivative of the deflection. Using (2.13) and (2.14), the load required to bend the beam to a radius R equal to that of the indentor is found to be

/>=4§[,

(2.15)

which indicates that wrapping is more likely to occur for long flexible beams under a large impactor. As the load increases, the beam comes in contact with the indentor over a distance a (Fig. 2.5). In that region, the radius of curvature is constant and equal to the radius of the impactor. Equation (2.13) implies that the bending moment is also constant, and (2.10) indicates that the shear force is uniformly equal to zero and that the pressure under the impactor is also zero. The beam is then loaded by two concentrated forces of magnitude P/2 located at +a and —a. The distance a is such that the curvature of the beam at x = a is equal to the

2.3 Indentation of Beams

11

Table 2.1. Analytical studies of contact between a beam and a rigid indentor Boundary conditions Simply supported

Indentor shape

Material Isotropic

Cylindrical

Orthotropic

Cylindrical

Clamped-clamped

Isotropic

Cylindrical

Cantilever

Orthotropic Isotropic

Cylindrical Cylindrical

Orthotropic

Flat Cylindrical Flat

Reference Keer and Miller (1983b) Sankar and Sun (1983) Shankar(1987) Sankar (1989a,b) Keer and Ballarini (1983a) Sun and Sankar (1985) Keer and Miller (1983b) Sankar and Sun (1983) Keer and Ballarini (1983a) Keer and Silva (1970) Keer and Schonberg (1986a) Keer and Schonberg (1986a) Keer and Schonberg (1986b) Sankar (1989a) Keer and Schonberg (1986b)

Figure 2.5. Beam wrapping around the indentor.

curvature of the indentor. For a < x < L/2, the bending moment is given by (2.14), and using (2.13) we find

« = f-2fi

(2,6,

for values of P larger than that given by (2.15). The conclusion from this simple analysis is that, neglecting local deformations, as a concentrated contact force would produce radius of curvature smaller than the radius of the indentor, the beam is loaded by two forces separated by a distance 2a. When local deformations are included, the pressure distribution is expected to be such that the maximum pressure is reached close to the edge of the contact zone. Beam theory does not predict those local deformations, and various approaches have been used to address the problem (Table 2.1). These investigators used various methods to study the loading portion of the contact laws for either

12

2 Contact Laws

0

0

0.25

0.5

0.75

Nondimensional distance Figure 2.6. Pressure distribution under a cylindrical indentor in contact with a simply supported beam (p = 0, 0.2, 0.4, 0.6, 0.8). isotropic or orthotropic beams. Of particular interest in these studies is the pressure distribution in the contact zone. Sankar (1989a) gave results for simply supported beams of length / centrally loaded by a rigid cylindrical indentor of radius R. The nondimensional contact pressure is given by p = (1 - x2)hl

- )8(1 - Ax2)}

(2.17)

where x = x/c, with c being the radius of the contact zone. The nondimensional contact pressure is related to the actual pressure by P=

nbc

, .

(2.18)

with c = c/l,fi = 8.755c 4 , B = ^§f(///?) 3 and Dx = Ex/(l - v?2), £>2 = 2Z?2/(^i + ^2)- M a n ( i ^2 are the roots of the bi-quadratic equation SnA.4 - (25i2 + S66)k2 + S22 = 0.

(2.19)

The components of the compliance matrix of the material are defined as •311 =

— ,

S22=—,

£2

c .312 =

Vl2

- —

,

c ^66 =

* -—.

(2.20)

2.4 Indentation of Plates

13

For small values of the parameter p, the contact pressure follows a Hertzian distribution (Eq. 2.2), but as f$ increases, the pressure is distributed more towards the edge of the contact zone as predicted by the beam analysis as shown in Fig. 2.6. This discussion indicates that as the beam becomes more flexible, the pressure distribution under the indentor becomes significantly different than that between the same indentor and a half-space. While this phenomenon may not have a major effect on the contact law, it will significantly affect the stress distribution under the impactor and should be considered when attempting to predict impact damage. Many investigators have studied the contact between smooth indentors and beams with various support conditions (Table 2.1); the reader is referred to these studies for further details.

2.4 Indentation of Plates Similarly, several analytical studies of the contact between a smooth indentor and laminated plates have been published (see Table 2.2). Many times the plate was modeled as an homogeneous orthotropic plate, but in some of the latest studies, the laminate nature of the composite is considered to determine the effect of the stacking sequence and the material properties on the contact law. An analysis of the indentation of simply supported laminated plates under rigid spheres using three-dimensional elasticity theory (Wu and Yen 1994) indicates that the stacking sequence has little effect on the contact law confirming previous experimental results (Tan and Sun 1985, Yang and Sun 1982). The contact force is found to be roughly proportional to the transverse modulus of Table 2.2. Analytical studies of contact between a plate and a rigid indentor

Material

Indentor shape

Isotropic

Sphere

Essenburg(1962) Keer and Miller (1983c) Chen and Frederick (1993)

Transversely isotropic

Sphere

Sankar (1985a) Cairns and Lagace (1987)

Laminate

Sphere

Wuetal. (1993)

Laminate

Sphere

Wu and Yen (1994)

Laminate

Sphere

Suemasuetal. (1994)

Reference

2 Contact Laws

14

0

0.5

1

1.5

Indentation 10~4mm Figure 2.7. Contact law predicted by Wu et al. 1993. the composite and independent of the longitudinal modulus, which had been suggested earlier by Yang and Sun (1982) based on experimental observations. When the contact force is small, plate thickness has essentially no effect on the indentation law. The contact behavior is then essentially the same as that for the indentation of a half-space. For larger indentations, the contact area increases, significant deviations from Hertzian contact law are observed, and changes in pressure distribution are similar to those shown in Fig. 2.6. In that case, laminate thickness has a significant effect on the force-indentation behavior. Wu et al. (1993) studied the contact between a composite laminate and a cylindrical indentor and showed that as the contact force increases, the contact behavior changes from a small contact area stage to a large contact area stage. During the small contact area stage, the size of the contact zone increases slowly and almost linearly with the contact force. As the contact force increases above a critical value, the size of the contact zone increases dramatically, and the contact pressure distribution changes dramatically from an Hertzian-type distribution to a saddle-type distribution of the type shown in Fig. 2.6. This characterizes the beginning of the large contact area. In Fig. 2.7, the small contact area

2.5 Indentation of a Laminate

15

phase corresponds to the curve between the origin and point A. Beyond point A, the indentation actually decreases as the force keeps increasing because of this redistribution of contact pressure over a larger area. Wu and Shyu (1993) showed that the contact force for the onset of delamination is independent of indentor size and that indentation consists of two stages. In the small indentation stage, the plate is still intact and the stacking sequence has insignificant effect on the force-indentation relationship. For large loads, damage becomes important, and the force-indentor movement curves differ for different layups. The contact behavior during low-velocity impacts is the same as in static tests.

2.5 Indentation of a Laminate A more practical approach consists of determining the relationship between the contact force and the indentation experimentally. Sun and coworkers (DanJumbo et al. 1989, Gu and Sun 1987, Sun et al. 1993, Tan and Sun 1985, Yang -and Sun 1982) studied the static indentation of laminated composites. Typically, during impact the contact force increases to maximum value and then decreases back to zero. In some cases, multiple impacts and reloading occurs. Therefore, contact laws should include the unloading and reloading phases. During the first loading phase, the contact law closely follows Hertz's law of contact (2.8). The parameter n in that equation is usually determined experimentally, but it can also be estimated if the radius of the indentor and the elastic properties of the impactor and the target are known using (2.9), with R given by (2.3). E in (2.9) is given by (2.4), Ei being the transverse modulus of the composite. Poisson's ratio of the composite is often taken to be zero (Yang and Sun 1982) in (2.4). Equation (2.8) describes the contact law during the loading phase of the indentation process. However, permanent indentation occurs even at relatively low loading levels, and the unloading phase of the process is significantly different from the loading phase. This phenomenon was observed by Crook (1952) for the indentation of steel plates by spherical indentors. During the unloading phase, the contact law suggested by Crook is P = Pm[(a - ao)/(am - ao)]2\

(2.21)

where Pm is the maximum force reached before unloading, am is the maximum indentation, and a0 is the permanent indentation. ao is zero when the maximum indentation remains below a critical value acr. When am > acr, ao = am[l-(acr/am)i].

(2.22)

16

2 Contact Laws

During subsequent reloading, the reloading curve is distinct from the unloading curve but always returns to the point where unloading began (Yang and Sun 1982). The unloading curve is modeled by P = Pm[(a - ao)/(am - ao)]l

(2.23)

The parameter ao does not necessarily correspond to the permanent indentation of the laminate, even though (2.23) indicates that P = 0 when a = a0, ao is selected so that (2.23)fitsthe experimental unloading curve using a least squares fit procedure. The parameter <x0 is related to the actual permanent indentation ap and the maximum indentation am during the loading phase by ao = P(am-ap)

(2.24)

when am > a cr ; G?O = 0 otherwise. The permanent indentation ap and the parameter ft are determined from experiments. However, many experiments need to be performed in order to determine these parameters, whereas a single unloading curve is necessary to determine acr when (2.22) is used. Yang and Sun (1982) presented experimental results for glass-epoxy and graphite-epoxy laminates. The elastic properties of the glass-epoxy material system were Ei = 39.3 GPa,

E2 = 8.27 GPa,

Gl2 = 4.14 GPa,

v12 = 0.26. (2.25)

For the loading phase, the contact law follows (2.8); for a 6.35-mm-radius indentor, the experimentally determined contact law is />exp = 1.60 x 10 4 c^,

(2.26)

and the predicted contact law is />pred = 1.90x lO 4 *!.

(2.27)

The critical indentation is 0.1016 mm (.004 in.). Figure 2.8 shows the loading curve given by (2.26) up to a maximum indentation of 0.3 mm and the corresponding unloading curve obtained from (2.21) and (2.22). If the indentation remains under 0.1016 mm, the unloading curve is identical to the loading curve, and as the maximum indentation becomes larger, the difference between loading and unloading paths is more pronounced. The area under the loading curve is the energy used to indent the laminate and is given by

U = ^JfcaL.

(2.28)

The area under the unloading curve is the energy recovered during the unloading

2.5 Indentation of a Laminate

17

3,000

2,500

2,000

1,500O LL 1,000-

500

0

i

0.05

0.1

i

0.15

I

0.2

r

0.25

0.3

Indentation (mm) Figure 2.8. Indentation of glass-epoxy laminate from Yang and Sum (1982). (a) Loading; (b) unloading; (c) reloading. process and is calculated using 2 7J

~

(2.29)

Cto)

For the case shown in Fig. 2.8, the ratio U'/U = 0.463 indicates that only 46.3% of the energy stored during the indentation process is recovered during unloading. This explains why, during the impact of a rigid structure where most of the impact energy is used for local indentation, the loading and unloading parts of the contact force history are significantly different. The reloading curve given by (2.23) is also shown in Fig. 2.8. After a first loading and unloading cycle, the target appears to be stiffer. Tests conducted on graphite-epoxy specimens with elastic properties Ei = 120.7 GPa,

E2 = 7.93 GPa,

Gn = 5.52 GPa,

v12 = 0.30 (2.30)

showed that the critical indentation was 0.0803 mm (3.16 x 10~3 in.).

2 Contact Laws

18

80

120

160

Maximum force (kN) Figure 2.9. Permanent indentation versus maximum contact force for the Kevlar-epoxy laminate tested by Meyer (1988). Meyer (1988) tested Kevlar-epoxy laminates with elastic properties Ex = 35.4 GPa,

E2 = 22.0 GPa,

vn = 0.175,

Gn = 7.36 GPa. (2.31)

A 15 cm x 15 cm x 2 cm piece cut from a cylindrical missile motor case with a 92.2 cm radius was continuously supported by a 92.2 cm steel platen and indented by a 25.4-mm-radius spherical indentor. The loading portion of the contact law is modelled by the equation P = 26 x l O V 2 5 .

(2.32)

During the unloading phase the behavior is modeled by

P=

Pm[{a-ao)/(ctm-ao)f

(2.33)

where the permanent indentation ao was shown to increase with the maximum load Pm (Fig. 2.9), and the exponent q has an average value of 4.1. It must be noted that the exponent in (2.32) is 2.25, compared to 1.5 for Hertzian contact,

2.6 Elastoplastic Models

19

Table 2.3. Experimental studies of contact Sun (1977) Lin and Lee (1990a) Leeetal. (1989) Meyer (1988) Sunetal. (1993) Cairns (1991) Swanson and Rezaee (1990) Wu and Shyu (1993) Yang and Sun (1982) Tan and Sun (1985) Dan-Jumbo et al. (1989) and that q = 4.1 for this Kevlar-epoxy laminate whereas for glass-epoxy and graphite epoxy the usual value is 2.5. The contact laws presented in this section are used extensively in the dynamic analysis of the impact event. Further experimental studies of contact can be found in the references listed in Table 2.3. 2.6 Elastoplastic Models With composites, permanent deformations are introduced when the indentation exceeds a small critical value. The material behavior in the transverse direction is governed by the properties of the matrix, and plastic behavior can be expected. Several investigators presented simple analyses for the indentation of a thin layer bonded to a rigid substrate (Cairns 1991, Christoforou 1993, Christoforou and Yigit 1994, Conway et al. 1970). First, the material is assumed to behave elastically until a critical indentation is reached. Then, the contact area is divided into a plastic zone and an elastic zone as the loading increases and a new contact law is obtained. Consider a laminate of thickness h, supported by a rigid substrate and indented by a rigid sphere of radius Rt (Fig. 2.10). The indentation is assumed to occur as if the material immediately under the indentor was subjected to uniaxial compression in the z-direction and the deformation takes place as shown in Fig. 2.10a. From that figure, the indentation a can be written in terms of the radius of the sphere, R(, and the contact radius, Rc, as a = Ri-(Rf-Rl)*.

(2.34)

The contact radius can be expressed as Rc = (2aRt -a2)1*.

(2.35)

20

2 Contact Laws

(b)

Figure 2.10. Indentation of thin layer supported by arigidsubstrate. In general, the indentation is much smaller than the radius of the indentor; considering the simplification made in this analysis, the second term on the right-hand side of (2.35) is neglected, yielding i.

(2.36)

The displacements under the indentor can be written directly from Fig. 2.10b as 8(r) =a-

R(

(2.37)

For small indentations, the contact radius is much smaller than the radius of the indentor, and the bracketed quantity can be simplified so that a-^-.

(2.38)

The transverse normal strain is assumed to as uniform through the thickness and is given by ezz = 8(r)/h. Assuming that the material behaves elastically, the contact force is given by P =

r

8(r)rdr,

(2.39)

2.6 Elastoplastic Models

21

Strain Figure 2.11. Stress-strain relations for elastoplastic analysis. where E is the modulus of elasticity in the transverse direction. Using (2.36) and (2.38), Eq. (2.39) gives the contact law (2.40)

for elastic contact. The model indicates that the contact force increases with a2 instead of a3/2, as predicted by Hertz law of contact. Permanent indentations are observed even for low values of the contact force. To account for these effects, assume that in the transverse direction the stressstrain behavior of the composite material is elastoplastic (Fig. 2.11). Because deformations are larger at the center of the contact zone, stresses will reach the yield strength first in the center, and the contact area can be divided into a plastic zone of radius Rp and an elastic zone between Rp and Rc. At the junction between the two zones, the stress is equal to the strength of material Zc so that Zc = j

(2.41)

Using (2.38), we find the radius of the plastic zone as (2.42)

as long as the indentation a is larger than the critical indentation Zch

acr. During the unloading phase, it is assumed that for r < Rp, the material will follow the elastic unloading path shown in Fig. 2.11 and that the stress-strain relation is given by cr = Zc + E(€-em). (2.46) The contact force during the unloading phase is given by P = 7tRiZc with Rp = [2Rt(am - Zch/E)]l/2.

After integration, (2.47) gives the contact

2.6 Elastoplastic Models

23

0 0

0.5

1

Indentation (mm) Figure 2.13. Comparison of experimental results with predictions of elastoplastic analysis (Eqs. 2.40, 2.45, 2.48). law for unloading TtRiE

(2.48)

for a > oio, with the permanent indentation ao defined as (2.49) Swanson and Rezaee (1990) conducted indentation tests on carbon-epoxy [0,±68,0]s laminates supported by rigid platen. The elastic properties of the material are Ex = 169 GPa,

E2 = 6.72 GPa,

v12 = 0.266,

Gn = 5.26 GPa, (2.50)

the thickness of the laminate is 2.4 mm, and the diameter of the indentor is 15.88 mm. The Hertz law of contact can adequately model the loading phase but for large loads (above 36,000 N), contact laws deviate significantly from Hertz law during the loading part of the indentation process. That smooth deviation is attributed to severe damage introduced during indentation of specimens that are back-supported by a hardened steel block. Figure 2.12 indicates that for

24

2 Contact Laws

these load levels the indentor has penetrated more than half the thickness. The elastoplastic analysis also provides a reasonable fit to the experimental data as shown in Fig. 2.13. 2.7 Conclusion It is generally accepted that for most current material systems such as graphiteepoxy or glass-epoxy, the indentation of a composite structure can be modeled using a statically determined contact law. The loading, unloading, and reloading portions of the force-indentation curves are modeled using (2.8), (2.21)-(2.23) with parameters usually obtained from experiments. Various aspects of the contact problem have been examined in details both experimentally then analytically, but these equations are now used by most investigators in mathematical models for the analysis of the impact dynamics.

2.8 Exercise Problems 2.1

Plot the loading phase of the contact laws for glass-epoxy, graphite-epoxy, and Kevlar-epoxy laminates under a 10-mm-radius indentor as the contact force increases from 0 to 1000 N. The material properties for these materials are given by (2.25), (2.30), and (2.31), respectively. 2.2 For the three materials in problem 2.1, plot the size of the contact zone and the maximum contact pressure as a function of the contact force. Discuss implications for stress distribution in the contact zone. 2.3 Starting with the Hertzian contact law, derive an expression for the energy required to produce a maximum indentation a max . What would be the energy needed if the contact force increases linearly to the same maximum level? 2.4 Consider a simply supported rectangular steel beam indented by a steel sphere. The indentation is expected to follow the Hertz law of contact. Find the overall deflection of the beam and the local indentation, and discuss the relative magnitude of these two deformations. When is one negligible compare to the other? 2.5 When unloading is governed by (2.21), derive an expression for the energy recovered during the unloading process. 2.6 Many investigators neglect local indentation altogether, and others assume that both the loading and the unloading phases are governed by Hertz law and obtain excellent agreement with experimental results. Discuss when local indentation effects can be neglected and when they must be considered, and to what extent.

2.8 Exercise Problems 2.7

25

Thermoplastic composites are known to be more damage resistant. Explain how a lower transverse modulus would affect the contact stiffness, the size of the contact area, the pressure distribution under the indentor, and therefore impact resistance.

3 Impact Dynamics

3.1 Introduction A first step in gaining some understanding of the effect of impact by a foreign object on a structure is to predict the structure's dynamic response to such an impact. Predictions are made using a mathematical model that appropriately accounts for the motion of the projectile, the overall motion of the target, and the local deformations in the area surrounding the impact point. In general, details of the local interaction between the projectile and the target are not needed to predict the contact force history. A particular beam, plate, or shell theory is selected, and the local deformation in the through-the-thickness direction, which is not accounted for in such theories, is included through the use of an appropriate contact law. Contact laws relate the contact force to the indentation, which is the difference between the displacement of the projectile and the displacement of the target at the point of impact. With most low-velocity impacts, small amounts of damage are introduced in a small zone surrounding the impact point, and the dynamic properties of the structures usually are not affected by the presence of damage. Therefore, impact dynamic analyses generally do not attempt to model damage as it develops during the impact event. The choice of a particular structural theory must be based on careful consideration of the effect of complicating factors such as transverse shear deformation and rotary inertia. For example, for beams, one can select to use the BernoulliEuler beam theory, the Timoshenko beam theory, or one of several other available beam theories. Similar choices are available for plates and shells, and the structure also can be modeled as a two- or three-dimensional solid. In this chapter, we will first present brief derivations of several beam, plate, and shell theories outlining the basic assumptions. Results from these different models are compared using static loading examples, free vibration examples, and wave propagation examples.

26

3.2 Beam Theories

27

Exact solutions to the equations of motion are available for some special cases of beams, plates, and shells subjected to dynamic loading. These solutions can be used effectively, but generally, approximate solutions must be sought. The finite element method is used often because it can be readily applied to a wide range of geometries and boundary conditions. Variational approximation methods are also used since in some cases they can provide more efficient solutions. The implementation of such methods, particularly with reference to the impact problem, is also discussed at length. To reduce cost, often tests are performed on small specimens rather than on full-scale prototypes. Whether such a scaling is possible and how to relate the results obtained on a small-scale model to the expected results on a full-scale model are also discussed in this chapter. 3.2 Beam Theories In this section we present the basic assumptions and the development of three beam theories: a higher-order theory, the Timoshenko beam theory, and the Bernoulli-Euler beam theory. Results from these theories for static loading, free vibration, and wave propagation examples will be compared in order to determine the applicability of each theory. 3.2.1 Bending of a Beam by a Uniform Load The following example, treated as a two-dimensional elasticity problem without any assumptions for a particular beam theory, is discussed to bring some understanding about the general behavior of beams, insight into why some of the assumptions in the various beam theories are made, and an understanding of each theory's limitations. Consider an isotropic beam of narrow rectangular cross section supported at the ends and subjected to a uniformly distributed load q (see Fig. 3.1). For this two-dimensional problem, the theory of elasticity (Timoshenko and Goodier 1970, pp. 46-48) indicates that the three nonzero stress components are 2/ V3~

2/

10*7

21*"

~

""" '

(3 la)

'

3 Impact Dynamics

28

Z

TTTTTTTT q

Figure 3.1. Simply supported beam subjected to uniform loading. where / is the moment of inertia of the beam. Equation (3.1c) indicates that the transverse shear stress axz follows a parabolic distribution through-thethickness of the laminate. The first term in (3.1a) represents the linear distribution through-the-thickness of the normal stress oxx that is predicted by the elementary beam theory. The second term in (3.1a) is the correction due the effect of the transverse normal stress azz, given by (3.1b). The normal stress axx reaches a maximum at x = 0 and z = h/2, at that point the second term in (3.1a) is less than 1% of the first term when L/ h > 2.58. Therefore, for most beams this correction term can be neglected, and the elementary beam theory is sufficiently accurate for most applications. In addition (3.1b) indicates that the transverse normal stress ozz is independent of x and has a maximum value of q at the bottom of the beam. The maximum value of ozz is less than 1% of the maximum value of oxx when L/h > 5.8. Therefore, for most beams this stress component is very small, its contribution to the total strain energy is small, and its effects are neglected in most beam theories. From two-dimensional elasticity, the displacements at an arbitrary location are u = 2EI h2

(3.2a)

v = —- 2EI h2x2 2EI

~2

12

(3.2b)

where u is the axial displacement; v is the transverse displacement; and 8 is the

3.2 Beam Theories

29

transverse displacement of the center of the beam (x = z = 0), which is given by 5 qLA where v is the Poisson's ratio for the material. The factor before the brackets in (3.3) is the deflection predicted by the elementary beam theory, and the second term inside the bracket represents the effect of shear deformation. As the ratio L/h becomes large, the effect of shear deformation becomes small. For a typical value of v = 0.3, this correction factor is less than 0.01 when L/h > 15. Therefore, for long beams the effect of shear deformations can be neglected as in the elementary beam theory. In the beam theories to be discussed here, the transverse normal strain is neglected, and the three theories differ in the way shear deformation is accounted for. With the higher-order theory, the transverse shear strain is assumed to follow a parabolic distribution and vanish on the top and bottom surfaces, as suggested by (3.1c). With the Timoshenko beam theory, the transverse shear strain is assumed to be constant through-the-thickness; with the Bernoulli-Euler beam theory (also called the elementary beam theory), the effect of transverse shear deformation is ignored altogether. 3.2.2 Higher-Order Beam Theory The development of the present higher-order beam theory is based on two hypotheses: (HI) The transverse shear strain vanishes on the top and bottom surfaces and follows a parabolic distribution through-the-thickness. (H2) The transverse normal strain can be neglected. These two hypotheses can be expressed as du dw ( 4z2\ ^z = 7 - + T - = y l - T T

.... ( 3 - 4a )

dw ezz = — =0 (3.4b) dz where y is the magnitude of the shear stress along the jc-axis. Equation (3.4b) yields w = wo(x), (3.5) and, after substitution into (3.4a), the axial displacement can be expressed as 4z3 u = uo(x) + z(y - wo,x) - — y.

(3.6)

30

3 Impact Dynamics

Considering only bending deformations (uo(x) — 0), and introducing the new variable \/r = y — wOiX, we obtain u = z^-^(f

+ wo,x).

(3.7)

From this equation, a physical interpretation of the function *I> is that it represents the rotation of a small line segment initially perpendicular to the jc-axis at z = 0. Equations (3.5) and (3.7) are the kinematic assumptions of the theory from which we get the two nonzero strain components du 4z3 txx = — = Zty, x - X77(V' + ™o,x),x dx 3hz

z2\

(

}

The strain energy, kinetic energy, and potential energy of the external forces are given by

U = \ [ (axxexx + 25. So far, this example indicates that shear deformations have a significant effect on the deflections for short beams and that this effect is more pronounced for composite beams. Now let us compare the stress distributions predicted by the beam theories with the elasticity solution. With the Bernoulli-Euler model, substituting (3.22) into (3.19b) and using Hooke's law, the axial stress is CTrx

=

(3.27)

3.2 Beam Theories

35

which is just the first term in (3.1a). The Timoshenko beam theory yields the same expression for the axial stress (3.27) and the following expression for the transverse shear stress: axz = —±-x. KA

(3.28)

With the higher-order theory, the transverse shear stress is

which is, for a rectangular beam, the exact result from the theory of elasticity. This indicates that the higher-order beam theory gives a much better prediction of the transverse shear stresses. The drawback is that the corresponding equations of motion and the boundary conditions are more complex than with the other theories. 3.2.6 Recovery of Accurate Stresses from Beam Models If an accurate determination of the transverse shear stresses is needed, it is possible to use the simpler elementary beam theory to determine the axial stress and then to use this result to determine the shear stresses from the equations of equilibrium of two-dimensional elasticity. For example, with the simply supported beam under uniform loading, the axial stress is accurately predicted (3.27) by the Bernoulli-Euler beam theory. Considering the beam as a two-dimensional solid, in the absence of body forces, equilibrium in the x-direction is governed by ^ I + ^i=0. ax dz From (3.30), the shear stress at location z is given by °zx X,Z - J

(3.30)

(3.31)

Substituting the expression for axx obtained from the Bernoulli-Euler beam theory (3.27), we find

which is precisely the exact solution for a rectangular beam obtained from the theory of elasticity (3.1c). Similarly, from two-dimensional elasticity, the equation of equilibrium in the z-direction is ^ + ^ = 0 . dx dz

(3.33)

36

3 Impact Dynamics

Integrating through-the-thickness from the bottom of the beam to an arbitrary location z, we obtain (J«(JC,

z)+q = - I' J_|

dGxz{ Z

^ ^dz\ dx

(3.34)

Substituting the value of the shear stress given by (3.32), the exact value of the transverse normal stress given by (3.1c) is recovered from (3.34). Therefore, it is possible to accurately determine both the transverse normal stress and the transverse shear stress distributions from the results of the elementary beam theory. 3.2.7 Harmonic Wave Propagation In order to compare the dynamic behavior of beams described by the three theories previously discussed, consider the propagation of free harmonic waves of the form w = We1"***-"0,

ir = W ^ - * 0

(3.35a,b)

where k is the wavenumber and co is the frequency. The wavenumber is related to the wavelength of the disturbance by k = In /A., and the phase velocity is c = co/k. Studying the propagation of free harmonic waves in an infinite beam allows us to gain some understanding about the dynamic behavior of the beam. Substituting w from (3.35a) into the equation of motion for a BernoulliEuler beam (3.20) gives co2 = ^jk4, or in terms of the phase velocity, c = (^j)l^2k. This indicates that beams are dispersive because the phase velocity depends on the wavelength, and that waves with shorter wavelengths propagate faster than waves with longer wavelengths. With this beam theory, however, short wavelengths can propagate with infinite speeds, which is not physically possible. This problem is the direct result of the simplifying assumptions made in the development of that theory. Substituting (3.35) into the equations of motion of a Timoshenko beam (3.16) gives the system of homogeneous equations:

K

» H-^[Ml1 2i

where A'n = KGAJC2, Mn = pA,

K22\

*]){W}=0

[M2l M22\)\V\

K22 = KGA + Elk2,

M22 = pi,

M

K12 = -K2\ = iicGAk,

M\2 = M2\ = 0.

(3.36) K } (3.37)

For nontrivial solutions, the determinant of the matrix of the coefficients in

3.2 Beam Theories

37

(3.36) must vanish, which gives the dispersion relation

pApIco4 - o)2[pA(EIk2 + KGA) + tcGApIk2] + tcGAEIk4 = 0.

(3.38)

This equation shows that for a given value of k there will be two solutions for the frequency or phase velocity. Plots of phase velocity versus wavenumbers are called dispersion curves, and in this case we will have two branches. For very long wavelengths, k approaches zero and (3.38) gives the two cutoff frequencies co\ = 0, o>i = (GA/pI)l/2. The first branch corresponds to bending motion, and the second branch to shear deformation. It can be shown that a first approximation to the first branch is co2 = ^jk4, which means that for long wavelengths the Timoshenko beam theory will predict the same behavior as the elementary beam theory. For short wavelengths (large values of k), Eq. (3.38) implies that the phase velocities tend to two limiting values: d = (icGA/pA)l/2,C2 = (El/pi)1/2. Therefore, the phase velocities are bounded for short wavelengths. The equations of motion of the Timoshenko beam can be written as uncoupled: EIwyXXXX + pAwjt - \pl + pA—— KGA\ [ EIf,xxxx

w,xxtt H

+ pAyjf,tt - \pl + pA—— 1, L KGA\

——Wjttt = 0

(3.39)

KGA tXXtt

+ £-A-^ KGA

=

o.

(3.40)

Abramovich and Elishakoff (1990) neglected the wJttt terms in these equations and obtained solutions to free and forced vibration problems. For free wave propagation, the effect of this simplification is to remove the pA pi co4 term from the dispersion equation (3.38). In that case, there is only one branch of the dispersion curve, and the phase velocity tends to the limit £ = (|y + ^ ) 1 / 2 for short wavelengths. After substituting (3.35) into the equations of motion for the higher-order beam theory (3.11), the dispersion relations are given by (3.36) with

K

a

" ' ^ ; ~ = pA H k ,

16 A/12 = —plki,

M

105

2X

(3.4.)

68

M22 =

pi,

= -MX2.

The two cutoff frequencies for long wavelengths are co\ =0,oo2 = (^^j)1^2. The shear correction factor K used in the Timoshenko beam theory is now

38

3 Impact Dynamics

100

200

300

400

Wavenumber k Figure 3.3. Dispersion curves for a steel beam with rectangular cross section. Solid line: Timoshenko's beam theory; dashed line: Bernoulli-Euler beam theory; dotted line: higher-order theory. replaced by | | = 0.8235 in the expression for the second cutoff frequency. In many cases, K is taken to be | = 0.8225 for beams with rectangular cross sections. For short wavelengths, the phase velocity tends to limit c = (EI/pI)l/2 for both modes. Example 3.1: Wave Propagation in Isotropic Beam To compare the three beam theories, consider the example of a steel beam with E = 210 GPa, v = 0.3, h = b = .05 m, p = 7850 kg/m3. For A: < 100, the higher-order theory and the Timoshenko beam theory give very similar results (Fig. 3.3). The higher-order theory will not bring about drastic changes in the predictions of the dynamic behavior of the beam. For the first mode, the phase velocity predicted by the Timoshenko beam has nearly reached its asymptotic value of 2928 m/s when k = 400, while with the higher-order theory the phase velocity keeps increasing to eventually reach a much higher asymptotic value of 5172 m/s. Figure 3.3 also shows the results obtained from the Bernoulli-Euler beam theory which

3.2 Beam Theories

39

indicate that this theory is applicable only for very long wavelengths k or small values of k{k = InIX). 3.2.8 Free Vibrations of Beams Another way to study the dynamics of the various beam theories is to study the free vibrations of finite beams. The natural frequencies of a simply supported beam of length L are identical to the frequencies of free harmonic waves with wavenumbers k = in/L. The study of harmonic wave propagation indicated that differences between the Timoshenko beam model and those from the higher-order theory are small. Therefore, the higher-order theory will not be considered in this section. Exact solutions for simple beams with any combination of boundary conditions at the ends will be developed for both the Bernoulli-Euler and the Timoshenko beam theories. An example of a clampedclamped beam will be used to illustrate the effect of the slendemess ratio, shear deformations and rotary inertia on the natural frequencies. For free vibrations of a Bernoulli-Euler beam, the displacements are taken in the form w(x, t) = W(x) sin(a)t).

(3.42)

Substituting (3.42) into the equation of motion (3.20) gives the ordinary differential equation dW El—- 4 dx

pAa)2W = 0.

(3.43)

Seeking a solution of the form W = e^*^, we find by direct substitution that (3.43) is satisfied for four distinct values of P*

ft = iP, fi = -iP, where fi = (co2pA/EI)l/4. form

P*3=P,

PZ = -P

(3.44)

This indicates that the general solution is of the

W(x) = A sin px + B cos fix + C sinh fix + D cosh

fix

(3.45)

where the constants A, B, C, and D have to be determined from the boundary conditions. Since there are two boundary conditions at each end of the beam, using (3.45), a system of four equations of the form

(3.46)

40

3 Impact Dynamics

will be obtained. For each of the natural frequencies of the beam, the determinant of the matrix K vanishes so that a nontrivial solution can be obtained for the four constants A-D. Therefore, the natural frequencies for beams with any combinations of natural frequencies at the ends can be determined by finding the zeroes of a 4 x 4 determinant. Exact solutions for the free vibration of Timoshenko beams are obtained by substituting w = WePx sin cot,

f = Xtfix sin cot

(3.47)

into the equations of motion (3.16), which leads to

Uf

+ pAa?)

GAP 2

[

- pico +

]]IW\-0 GA)\

)\ \ X J ~

a

Nontrivial solutions are obtained when the matrix of the coefficients vanishes, which implies that fi satisfies the bi-quadratic equation

^"4

GAEI

El

"2 °

^

This equation will have two solutions with the corresponding mode shapes

where 0 n = -GAjSi, 02i = —GAfc, The general solution is

0i2 = GApl + pAco2 , , 022 = GAfy + pAco .

W = A(pn sin^ix + Bcpn

(3-51)

COS^IJC

+ C(p2\ sinh p2x + C^2i cosh fax X = A2

El

-12 -6L 12

6L

(2 - 0)L2 -6L

(4 + 0)L

symmetric

(3.53)

2

where

0

12 / E I \ L 2 \KGA '

(3.54)

The mass matrix is the sum of two matrices: the matrix associated with translational inertia

[MpA] =

pAL

^22

^23

21O(l+0) 2

(3.55)

m34

symmetric

W44J

with

mu = m33 = 7O02 + 1470 + 78,

m12 = (3502 + 770 + 44)-,

4 mu = - ( 3 5 0 2 + 630 + 2 6 ) - , 4 (3.56) L2 L = m44 = {Icf)2 + 140 + 8) — , m23 = (350 2 + 630 + 2 6 ) L2 L 2 = - ( 7 0 + 140 + 6) — , m34 = - ( 3 5 0 2 + 770 + 4 4 ) - ,

mn = 350 2 + 630 + 27, m22 m24

and the matrix associated with rotatory inertia

[MpI] =

^22

3O(1+0) 2 L

^23

^24

m33

m34

(3.57)

symmetric m n ~~ ^13

==

^33 ~~ 36,

mi2 = mi4 = —^3

m22 = m44 = (1O02 + 50 + 4)L 2 , 2

4

==

—(150

— 3)Z^,

m23 = - ( 1 5 0 - 3)L,

(3.58)

2

m24 = (50 - 50 - 1)L . To ascertain the accuracy of that finite element, consider the error in the eigenvalues obtained using uniform meshes with increasing numbers of elements.

3.2 Beam Theories

43

The error is defined as (3.59) where the subscript / denotes the /th natural frequency and the superscript E indicates the exact value of the natural frequency or eigenvalue. Example 3.3: Convergence of Finite Element Analysis of Beam Vibrations The example treated by Friedman and Kosmatka (1993) is a simply supported beam with £7 = 1,

pA = l,

h/L = 0.2,

v = 0.3

(3.60)

with the shear correction factor 10(1 + v) K

=

Because of symmetry, only half of the beam needs to be modeled. Figure 3.5 shows that the error varies with h2, h being the length of one element-or 1E+00

1E-01

1E-02

1E-03

LJJ 1E-04-

1E-05-

1E-06 4

40

Number of elements Figure 3.5. Modelization error in finite element analysis of free vibration of beams.

44

3 Impact

Dynamics

Table 3.1. Natural frequencies of simply supported beam Mode

1 2 3 4 5 6

32 Elts.

Exact

Error

9.28200 32.24894 61.72164 93.81159 126.88143 160.26995

9.281920 32.24561 61.69867 93.73128 126.6825 159.8679

1.767e-5 2.066e-4 7.447e-4 1.714e-3 3.143e-3 5.036e-3

in other words, E varies with N 2, N being the number of elements in the discretization. As expected, the error increases for higher modes. Table 3.1 shows the accuracy of the first six natural frequencies obtained using a uniform mesh with 32 elements.

3.2.9 Effect of Geometrical Nonlinearities Since many composite structures are thin and flexible, moderately large deformations can be expected during impact. The effect of membrane stiffening on the impact dynamics and the contact force history should be investigated. Large displacements induce a coupling between axial and transverse displacements. For a Bernoulli-Euler beam, the kinematic assumption is written as u = uo —

(3.62)

zw;

where uo is the axial displacement and w is the transverse displacement. For moderately large displacements the axial strain is given by 1

l

-W

2 x.

(3.63)

When the material follows Hooke's law, the strain energy in the beam is given by

*xx}dx. +EIw*

(3.64)

The kinetic energy stored in the beam is given by T

= ? / [("« - z ^ * ) 2 + «£] dV = 1 / [PA(u2o + w2) + plw2x] dx. ^ JO

^ JO

(3.65) (365)

3.2 Beam Theories

45

Hamilton's principle (3.10) is used to derive the equations of motion l

(

i\

EA I uOjX + - w x I

= pA uo

f uo,x + -w2x )w,x\ ~ EIw,xxxx L\ ^ / J ,x and the boundary conditions where either EA

u

or

or

+ +

-EAluOjX or

= 0

w

-EIw,xx

(3.67) 1

- EA ( M

EIwxxx

(3.66a,b)

- pAw + pliv,xx

are prescribed at the ends. Since the effects of inplane inertia and rotary inertia are usually negligible, the right-hand side of (3.66a) and the pi term in (3.66b) are neglected, and the equations of motion now read = 0 x

EIwxxxx

+ pAih = EA

x

-,

(3.68a,b)

I uo,x + -w

Integrating (3.68a) gives *o,x + ^2X

= C{f).

(3.69)

w\dx.

(3.70)

Integrating again gives C(t) = ^-

f

After substitution into (3.68b), \ EA ( fL EIw,xxxx + pAib = —— I / w 2xdx w,xx. (3.71) lL \Jo ' / For simply supported beams, a one term Rayleigh-Ritz approximation can be obtained by taking w = a sin — . (3.72) Li

Substituting into (3.71), multiplying by sin ^ , integrating over the length of the beam, and using the change of variables r = cot, where a? = (f ) 4 ^ , yields the well-known Duffing equation: a + a + ea3 = 0

(3.73)

3 Impact Dynamics

46

— Exact --RR1

6-

4-

3

0

1

2

3

4

5

Amplitude / radius of gyration Figure 3.6. Effect of geometrical nonlinearities on the free vibrations of beams.

where _ A _ 1 (3.74) 4/ = 4 ^ and r is the radius of gyration of the cross section. Using the Linstedt-Poincare perturbation approach, the ratio of the nonlinear and linear fundamental frequencies is obtained as € =

coL

3 1 , 3 _2 = 1 + -€az = 1 + — 8 32 32

-\ 2

- I W

(3.75)

where a is the vibration amplitude. Figure 3.6 shows that when the amplitude remains small compared with the radius of gyration of the beam cross section, the nonlinear effects remain small and a linear model can be used. 3.2.10

Summary

Any beam theory is based on a set of assumptions aimed at reducing the threedimensional elasticity problem to a one-dimensional problem. In this section,

3.2 Beam Theories

47

we reviewed the basic assumptions made in the development of three basic theories: the Bernoulli-Euler beam theory, the Timoshenko beam theory, and a higher-order theory. The equations of motions and boundary conditions were derived from Hamilton's principle in a consistent way for each theory. The example of a simply supported beam subjected to a uniformly distributed load was used to compare the stresses and deflections predicted by the various beam theory to elasticity results. The objective was to evaluate the validity of the assumptions made in the development of the theories and to develop some general guidelines concerning the applicability of these theories. This example showed that for slender beams, the Bernoulli-Euler beam theory, which is the simplest of the three, provides very accurate results, but for shorter beams, the Timoshenko beam, which accounts for transverse shear deformations, is required. Shear deformation effects depend on the ratio of the elastic and shear moduli and therefore are more pronounced for composite beams, since the ratio is usually much higher for composites than for steel or aluminum. An analysis of harmonic wave propagation in beams shows that for most practical cases, the higher-order theory gives results that are very close to those predicted by the Timoshenko beam theory. Therefore, the increased complexity of the theory is not justified by any improvement in the results. Free vibration analyses show the importance of transverse shear deformation and rotary inertia on the dynamic behavior of beams. The effect of large deformations is investigated by considering the large-amplitude vibration of simply supported beams. Results show that as long as the amplitude remains small relative to the radius of gyration of the cross section, nonlinear effects are negligible. In many cases, impact tests are performed on beam specimens, and the beam theories discussed in this section will be used in the development of mathematical models for studying the impact dynamics. In addition, the knowledge about the various assumptions and the effects of shear deformations and rotary inertia gained through this study of beam theories will be directly applicable to the development of plate and shells theories examined in the following sections.

3.2.11 Exercise Problems 3.1

3.2

Using the Timoshenko beam theory, derive an expression for the static deflection of a cantilever subjected to a concentrated force P at the end. Show the effect of the slenderness h/L ratio on the magnitude of the shear deflection relative to the bending deflection. Following the approach shown Section 3.28, formulate the free vibration problem for a cantilever Bernoulli-Euler beam. Write down the four

48

3.3

3.4

3.5

3 Impact Dynamics boundary conditions in the form given by (3.46), and expand the 4 x 4 determinant to obtain the characteristic equation. Derive a beam theory neglecting the transverse normal strain and assuming that the transverse shear strain varies as a cosine function of z that vanishes on the top and bottom surfaces and reaches a maximum for z = 0. Determine the axial stresses and the transverse shear stresses in a simply supported, rectangular, Timoshenko beam subjected to a sinusoidally varying distributed load that vanishes at both ends. Compare with the results obtained using the Bernoulli-Euler beam theory and determine the effect of shear deformation. Use the approach shown in Section 3.2.6 to determine the transverse shear distribution from the results of the Bernoulli-Euler beam theory. Write a computer program to calculate the natural frequencies of Timoshenko beams using the exact approach discussed in Section 3.2.7. 3.3 Plate Theories

From the discussion on the effect of shear deformation and rotary inertia on the static and dynamic behavior of beams, it is expected that these two factors will have similar effects on the behavior of plates, particularly for plates made out of composite materials. The first-order shear deformation theory (FSDT), also known as the Mindlin or Mindlin-Reissner plate theory, which is an extension of the Timoshenko beam theory, will be presented first. For thin plates, the effect of shear deformation and rotatory inertia are small, and the theory can be reduced to the classical plate theory (CPT), which is the equivalent of the Bernoulli-Euler theory for beams. Higher-order plate theories are also available and will be discussed. 3.3,1 First-Order Shear Deformation Theory Following the discussion on beam theory, the development of a plate theory following the lines of the Timoshenko beam theory proceeds by assuming that the transverse normal strain ezz is negligible and that the two transverse shear strains are constant through-the-thickness. These two assumptions, which can be written as €zz = — =0 €xz

= ^ dv

(3.76a)

+ ^

= yi

dw

*yz = T - + - 7 - = K2,

oz

(3.76b)

oy

(3.76C)

3.3 Plate Theories

49

imply that the displacements are of the form u(x, y, z) = uo(x, y) + z(y\ ~ wo,x) v(x, y, z) = vo(x, y) + z(y2 - wOtX)

(3.77)

w(x,y,z) = wo(x,y). The change of variables

gives the displacement field of the first-order shear deformation theory in its usual form: u(x, y, z) — uo(x, y) + zirx(x, y) v(x, y, z) = vo(x, y) + zfy(x, y)

(3.79)

w(x,y,z) = wo(x,y) where uo,vo, wo are the displacement components of a point on the midplane. y\rx and \//y are the rotations of the normal to the midplane about the y- and ~;t-axes respectively. Equations (3.79) are often postulated as an assumption on the kinematics of the deformation in which a line segment initially normal to the midplane of the plate is assumed to remain straight but not necessarily normal to the midsurface during deformation. The infinitesimal strain components, defined as du dv dw yy zz dx' dy' dz ' (3.80) du dv du dw dv dw ^ y = 9y + a ? €xz = lh + 3Jc"' €yz ~ ~dz + ~dy' can be evaluated from (3.79): duo dx ezz = 0,

d\fsx dx ' exy =

duo

yy

1

dvo

dvo

d\/sy

dy

dy

h"

(dilfx

'

d\lr^

The plate is subjected to a distributed load q over the surface, normal inplane force resultants Nn over a part of the boundary T\,NS over F2, moment resultants Mn and Ms over F 3 and F 4 respectively, and transverse shear Qn forces over F5. The inplane force resultants are defined as (N;,Ny,Nxy)= = / J

(a(a ,oxy Xi,

•

o-0.20

^ •

\

x

•-

^k,,-

I

I

I

I

2

4

6

8

I

I

I

10 12 14 16

Radius/thickness Figure 3.14. Displacements of infinite plate subjected to a step load.

boundaries. After that time, the response will be affected by the boundary conditions. A solution for finite-sized composite plates is presented now to investigate the effect of finite size and anisotropy. The distributed loading and the displacement functions for a shear deformable plate (FSDT) can be expanded into the double Fourier series

E m,n=l

qmn(

mnx a

Wmn(t) sm

w = m,n=l oo

Xmn(t)cos m,n=\ oo

m7tx

sin mitx . nny

mnx

> sin

nny b

(3.191)

sin——

nny

cos ——.

In this way, for a simply supported plate with symmetric layup and no bendingtwisting coupling, the boundary conditions (3.139)-(3.140) are satisfied.

3.3 Plate Theories

75

Substituting (3.191) into the equations of motion (3.110)—(3.112) yields for each mode the set of three ordinary differential equations [M] I Xmn \ + [K] lxmn

\ = I 0 V

[ Ym J

Ymn J

(3.192)

[ J

with the generalized mass and stiffness matrices given by (3.184). 3.3.8 Variational Models In general, exact solutions for the dynamic response of laminated plates are not available and variational approximation methods can be used. According to the first-order shear deformation plate (FSDT) theory, the strain energy in a laminated plate is given by (3.90). The constitutive equations (3.99) and (3.103) can be written in matrix form as

Q = Ay. With this notation, the strain energy in the plate can be written as

U = \ f [ejAeo + KTDK + 2CJBK] dQ + \ [ yTAydQ.

(3.194)

For a symmetric laminate, the B matrix is zero and the inplane and transverse motions are uncoupled. In addition, if the effects of shear deformation are neglected (classical plate theory), the last term in (3.194) can be neglected and the strain energy becomes KTDicd£2

U = 2

(3.195)

Jn

when only out-of-plane deformations are considered. Using (3.94), the kinetic energy for a symmetric plate subjected to transverse deformations can be written as

T= =

\ L {h{ij2°+/3^'+^

}dQ

(3 l96)

*

when the effect of rotatory inertia are neglected, h = 0, and only the first term is left in the integrand of (3.196). For plates subjected to a distributed pressure q in the transverse direction only, the potential energy of the external forces can be written as V = - f qwodQ.

(3.197)

76

3 Impact Dynamics

With the Rayleigh-Ritz variational approximation method, the transverse displacements are taken as N

where the approximation functions 0/ must satisfy the essential boundary conditions and where the c, are constants to be determined. Substituting (3.198) into (3.195)-(3.197) yields U = -cT 2

<S>friDi(x,y)=xm-lyn-i

(3.205a)

0,-Oc, y) = xmyn(x - a)(y - b)

(3.205b)

4>i(x,y) = xm+lyn(y-b)

(3.205c)

for FFFF, SSSS, and CSFS plates respectively. Abrate (1995e) study the free vibrations of rectangular plate with intermediate line supports. With r supports located along the lines x = a\, a2, • • •, &r and s supports along the lines y = b\, £2, • . . , b s the approximation functions were taken as

4>i(x, y) = xm+ayn+\x

r

s

j=\

k=i

- aYiy - b)8 JJ(JC - aj) JJ(y - bk).

(3.206)

Following the same approach, polynomial approximation can be developed for other geometries. For example, for triangular plates with one edge along the x-axis, the approximation functions can be taken as (Abrate 1996a) 0;(x, y) = xm-lyn+a(cy

- bxf [bx + (a - c)y - abf

(3.207)

where a, /3, and y account for the support conditions along the sides v = 0, cy — bx — 0, and bx + (a — c)y — a = 0 and are taken to be -1,0, 1 for free, simply supported, and clamped edges, respectively. Example 3.10: Free Vibration of Plate with Intermediate Line Supports Consider a graphite-epoxy square plate with simple supports along the four edges and line supports along the lines x = a/4 and y = a/2, where a is the length of theside. The elastic properties ofthe material are E\ = 181.0 GPa, E2 = 10.30 GPa, V12 = 0.28, Gn = 7.17 GPa. The natural frequencies are nondimensionalized as follows: Q2 = co2pha4/(DnD22)l/2. Thefirstsix natural frequencies for angle-ply laminates are given in Table 3.4 as a function of the fiber orientation. The approximation functions are taken as &(*, y) = xay?(x - a)(y -

78

3 Impact

Dynamics

Table 3.4. Natural frequencies of graphite-epoxy angle-ply, two-way-two-span square plates Fiber orientation (degrees)

0 15 30 45 60 75 90

Natural frequencies (rad/s)

57.52 63.74 70.80 75.09 81.64 86.16 85.17

63.00 70.53 81.41 92.65 110.4 116.5 101.5

103.3 123.3 158.3 147.0 135.3 127.1 130.5

124.2 145.7 161.4 162.0 159.4 152.3 132.1

168.6 170.6 170.5 198.8 202.4 160.8 142.9

171.4 175.4 188.7 237.5 224.4 186.8 154.4

Table 3.5. Natural frequencies of clamped, elliptical, isotropic plate

1 9x9 Lam* 2 9x9 Lam 3 9x9 Lam 4 9x9 Lam 5 9x9 Singh**

10.2158 10.2160 27.3774 27.4773 56.8004 56.8995 97.5989 97.5984 149.6378 149.66

21.2604 21.2601 39.4974 39.4976 71.5912 71.5902 115.6089 115.6084 171.0975 171.10

21.2604 21.2601 55.9758 55.9773 90.2352 90.2380 137.2739 137.2686 196.2046 198.55

34.8772 34.8786 69.8580 69.8557 113.2753 113.2661 164.3236 164.3248 229.8105 229.81

34.8770 34.8786 77.0367 77.0443 140.7441 140.7461 195.3101 195.3398 266.2457

39.771 39.7712 88.0479 88.0472 150.0907 150.0889 255.1315 255.0946 350.4704

*Lametal. (1992). **Singh and Chakraverty (1994). The first six natural frequencies have converged for the first four significant figures when an 8 x 8 approximation is used. That is, a and f$ vary from 1 to 8, and TV = 64 in the displacement approximation (3.198). Example 3.11: Free Vibration of Elliptical Plate For clamped, isotropic, elliptical plates, the approximation functions are taken as ;, the boundary conditions (3.208) yield four equations that must be satisfied simultaneously: 1 ( - k\ • SS - CC)

-k\ ( - k'2 • CC - SS)

-1 ( - l\ • SH + CH)

-k\ ( - JkJ • CH + SH)

k[ r

. (k 2 • CC - SS)

r

( - k 2 - SS - CC)

r

(k 2 • CH + SH)

(kr2 • SH + C H ) .

(3.209)

80

3 Impact Dynamics Table 3.6. Natural frequencies (rad/s) of aluminum beam

Mode (1) 1 2 3 4 5 6

Experimental (2)

Cantilevered beam (3)

H&J* (4)

Elastically supported (5)

122.7 766.86 2131.6 4157.8 6818.64 10019.1

148.912 933.203 2612.93 5120.11 8463.48 12642.2

131.5 790.1 2148 4176 6868 10065

122.683 797.393 2240.33 4294.40 6818.64 9890.68

*Hassiotis and Jeong (1995). where

k\ =

k[ =

k>2-

k r2

(3.210)

and SS = :

3/L),

CC = cos(ftL),

SH = sinh(#L),

CH = cosh(#L). (3.211) For nontrivial solutions, the determinant of the matrix of the coefficients must vanish. For a given set of spring constants, the natural frequencies and mode shapes can be determined by finding the zeroes of a 4 x 4 determinant. The support stiffnesses are selected to minimize some objective measure of the difference between predicted and measured values of a set of natural frequencies: (3.212) 1=1

where £2; is the measured natural frequency, i is the predicted value, and N is the number of modes considered. Example 3.12: Identification of Boundary Conditions for an Aluminum Beam In this example, a 25.4-mm-wide, 6.35-mm-thick, 495.3-mm-long aluminum beam of uniform cross section is assumed to be clamped at one end and free at the other. The modulus of elasticity and the density of the material are E = 11 MPa and p = 2210 kg/m3, respectively. The natural frequencies predicted using classical cantilever boundary conditions (Table 3.6, column 3) are significantly higher that the experimental values (column 2). At x = 0, the support provides

81

33 Plate Theories Table 3.7. Natural frequencies (rad/s) of composite plate

Mode (1) 1 2 3 4 5

Experimental (2)

Finite element (3)

Cantilever beam (4)

Elastically supported

399.3 1113 2507.3 3992.1 7012.0

453.6 — 2826.4 4193.2 7859.6

453.254 — 2840.50 — 7953.47

399.300 — 2527.58 — 7011.96

(5)

some flexibility, and the best values for the rotational and translational spring constants are found to be k[ = 732,560 N/m, k\ = 668 N • m/rad. Example 3.13: Identification of Boundary Conditions for a Composite Plate Proper modeling of the support conditions for composite plates subjected to impact loading has long been recognized as a problem needing attention. Exjperiments were conducted on 3-layer graphite-epoxy specimens with a ply thickness of 0.015 in. and a total thickness of 0.045 in. The width was 2 in., the length 6 in., and the measured material properties are E\ = 19.832 Msi, E2 = 1.603 Msi, v\2 = 0.314, Gu = 0.926 Msi, p = 0.058 lb/in.3. Specimens were clamped at one end, and the natural frequencies and mode shapes were determined experimentally. Free vibrations were studied using a finite element model with an 8 x 17 mesh of 4 noded isoparametric plate elements, assuming the specimen to be clamped along the edge x = 0. The predicted natural frequencies (Table 3.7, column 3) are significantly higher than those measured (column 2). Since the material properties are known accurately, the discrepancy is expected to come from imperfect boundary conditions. Experiments and finite element results indicate that, for this example, modes 1,3, and 5 are pure bending modes and modes 2 and 4 involve torsional motion. Results obtained using the Bernoulli-Euler beam theory with cantilever boundary conditions (column 4) show that the bending modes are predicted accurately and that shear deformation effects are small because the specimens are thin. The difference between the finite element results (column 3) and the cantilever beam results (column 4) is due to the effect of shear deformation. Using the present approach, the support at the root is modeled by two linear springs whose stiffnesses were determined by minimizing the error measure EB for the first three bending modes. Using k[ = 3595 lb/in. and k\ = 684.0 lb • in./rad, excellent agreement is obtained between experimental results in column 2 and the predicted frequencies in column 5.

82

3 Impact Dynamics 3.3.10 Summary

In this section, the derivation of three plate theories were reviewed: the classical plate theory, the first-order shear deformation theory, and a higher-order plate theory. One static example illustrated the fact that as the ratio between the length of the side and the thickness of the plate becomes small, shear deformation effects become significant. Loading a plate with a concentrated force creates a singularity at the point of application of that force, which results in slow convergence in the solution procedure. In practice, loads are introduced through a small patch, and under such a loading, convergence problems are avoided and realistic distributions of transverse shear forces are obtained. Harmonic wave propagation analysis confirms the effect of shear deformation and indicates that the effects of rotary inertia are small in the range in which the plate theory is applicable. The bending-twisting coupling terms have a significant effect with four-ply laminates but are negligible when there are eight plies or more. Since there are only a few cases of plates for which closed-form solutions can be found, a variational approximation method capable of handling many complex cases was presented. Actual boundary conditions are often different than the ideal conditions and will significantly affect the dynamics of the structure. A procedure to determine the actual boundary conditions has been presented. 3.3.11 Exercise Problems 3.6

3.7 3.8

3.9

3.10

Use a one-term polynomial approximation in the Rayleigh-Ritz method to determine the fundamental natural frequency of a rectangular, simply supported plate. Compare the results with the exact solution given by (3.182). Using the classical plate theory, derive an exact solution for the deflection of a simply supported plate subjected to uniformly distributed static load. Using the first-order shear deformable plate theory, derive an exact solution for the deflection of a simply supported rectangular plate subjected to uniformly distributed static load. Assume that the laminate layup is specially orthotropic. Investigate the effect of shear deformation as a function of the ratio between the length of the side of the plate and the thickness. Derive a one-term Rayleigh-Ritz approximation for the fundamental natural frequency of an orthotropic rectangular plates with all four edges fully clamped. Use a polynomial approximation function. Develop an exact solution for the deflection of a rectangular, simply supported plate subjected to a force applied in its center. Assume that

3.4 Impact Models

3.11

83

force is applied as (1) a concentrated force and (2) a uniform pressure applied on a small square patch centered at the center of the plate. Plot the displacements along one line of symmetry of the plate, and investigate the effect of patch size and the number of terms retained in the solution. Develop a solution for the dynamic response of a rectangular, simply supported plate subjected to step load applied in its center. Compare this solution with the solution given by Medick (Section 3.3.7) for the transient response of an infinite plate to the same load. Show that the solution for an infinite plate is valid for very short times. That is when the disturbance has not yet reached the boundary and reflected back.

3.4 Impact Models Several types of mathematical models are used to study the impact of a structure by a foreign object. In certain cases, the contact force history can be accurately determined by modeling the structure by an equivalent spring-mass system. When the structure behaves quasi-statically, it is also possible to calculate the maximum contact force by assuming that when the contact force reaches its maximum, the sum of the strain energy in the structure and the energy required for indentation is equal to the initial kinetic energy of the projectile. This energybalance approach is useful when one is interested not in the complete contact force history but rather only in maximum contact force. When the dynamics of the structure must be more accurately accounted for, more sophisticated models are needed. In this section, the various models used for impact analysis are discussed, and examples are presented to illustrate various features of the impact event.

3.4.1 Spring-Mass Models Spring-mass models are simple and provide accurate solutions for some types of impacts often encountered during tests on small-size specimens. The most complete model (Fig. 3.15) consists of one spring representing the linear stiffness of the structure (Kbs), another spring for the nonlinear membrane stiffness, a mass M2 representing the effective mass of the structure, the nonlinear contact stiffness, and Mi, the mass of the projectile. From the free body diagrams of the two masses Mi and M2, we obtain the equations of motion: rjci + P = o, mx2 + Kbsx2 + Kmx$ - P = 0.

(3.213)

84

3 Impact Dynamics

E

T' x2

T

Figure 3.15. Spring-mass model. P is the contact force which, as discussed in Chapter 2, is a highly nonlinear function of the indentation x\ — JC2, which can be expressed as P = P(Xl-x2)

(3.214)

when x\ > x2. When x\ < *2, contact ceases, P = 0, and (3.208) govern the free vibration of the model. The dynamics of the system described by (3.208) and (3.209) and the initial conditions *i(0) = V,

*i (0) = * 2 (0) = 0

(3.215)

can be studied numerically. When geometrical nonlinearities and the indentation are negligible, the model can be significantly simplified to a single degree of freedom system with the equation of motion M'x + Kbsx = 0.

(3.216)

In that model, the effective mass of the structure is neglected and the structure and the projectile move together as soon as contact is made (JCI = x2 = x). The general solution to (3.216) is x = A sin cot + B cos cot

(3.217)

where to1 = Kbs/M\. The constants A and B are determined from the initial conditions (3.215), which give the result V x = —sincot. CO

(3.218)

3.4 Impact Models

85

Since the contact force P is equal to the force in the linear spring Kbs, the contact force history is given by F = Kbsx = V(KbsMi)i

sincot

(3.219)

for cot < n. When cot > n (3.214) predicts a negative contact force, which is impossible because contact between the projectile and the structure is unilateral. Therefore, separation occurs for t = Tc = TT/CO. The contact duration Tc increases with the mass of the projectile and decreases as the stiffness of the structure increases: Tc = n(Mx/Kbs)l

(3.220)

Equation (3.219) shows that the maximum contact force is directly proportional to the impact velocity and also increases with both the square root of the stiffness of the structure and the square root of the mass of the projectile. The maximum contact force is often plotted versus the initial kinetic energy of the projectile. For a given projectile (3.219) predicts that the maximum contact force increases with the square root of the kinetic energy. Example 3.14: Impact on a Half-Space Consider the impact on a half-space made out of steel by a 10-mm-radius steel ball with an initial velocity of 10 mm/s. The mass of the impactor is 32.24 g, Young's modulus is taken as 215.8 GPa, the density as 7966 kg/m3, and the contact stiffness as 1.538 x 1010 N/m 3/2 . In this case, there is no overall deflection of the target, so the motion of the projectile is governed by (3.213), where x\ represents both the displacement of the projectile and the indentation of the half-space and P = kcxx . This nonlinear equation of motion was solved using Newmark's step-by-step integration method with a time step of 2 /xs. The contact force history is given by the solid line in Fig. 3.16. The contact duration is 170 /xs, and the maximum contact force is 6.96 N. Some investigators linearize the contact law in order to avoid numerically solving a nonlinear differential equation. In this case, taking P = Ka, the equation of motion of the projectile is given by (3.216), the contact force is given by (3.219), and the contact duration is given by (3.220), where Kbs is replaced by K. If K is determined from (3.219) so that the maximum contact force matches that determined numerically (K = 1.503 x 107 N/m), the contact duration is significantly underestimated (Fig. 3.16). If K is determined from (3.220) so that the contact duration matches the numerically determined contact duration (K = 1.101x107 N/m), the maximum contact force is severely underestimated (Fig. 3.16). Therefore, for impacts dominated by local indentation, the use of linearized contact laws leads to significant errors.

3 Impact Dynamics

86 87-

\

/ /

/ / / .*

6-

^^ ^^

5-

\

\

\

••••»

\ \ \*. \ ^* •\

/ /

90.

'/ 7/

4-

x x

'' • /

•' -7

o

LL 3 -

\

/ .7 ///

2-

/

'•' i K f

0

\ \

#. 1 - //

I 0 - !/ /

V

i

i

50

100

\

\ V• \ \\ 150

Time (/JS) Figure 3.16. Impact of a sphere on a half-space.

3.4.2 Energy-Balance Models Another approach for analyzing the impact dynamics is to consider the balance of energy in the system. The initial kinetic energy of the projectile is used to deform the structure during impact. Assuming that the structure behaves quasistatically, when the structure reaches its maximum deflection, the velocity of the projectile becomes zero and all the initial kinetic energy has been used to deform the structure. The overall deformation of the structure usually involves bending, shear deformation, and for large deformations, membrane stiffening effects. Local deformations in the contact zone also are to be considered. For impacts that induce only small amounts of damage, the energy needed to create damage can be neglected. Therefore, the energy-balance equation can be written as

where the subscripts b, s, and m refer to the bending, shear, and membrane components of the overall structural deformation, and Ec is the energy stored in the contact region during indentation. It is always possible to express the

3.4 Impact Models

87

force-deflection relation in the form P = KbsW + KmW3

(3.222)

where Kbs is the linear stiffness including bending and transverse shear deformation effects, Km is the membrane stiffness, and W is the deflection at the impact point. Then Eb + Es + Em= l-Kbs Wlm +X-Km

IMPACT ON COMPOSITE STRUCTURES

IMPACT ON COMPOSITE STRUCTURES SERGE ABRATE Southern Illinois University at Carbondale

CAMBRIDGE UNIVERSITY PRESS

CAMBRIDGE UNIVERSITY PRESS Cambridge, New York, Melbourne, Madrid, Cape Town, Singapore, Sao Paulo Cambridge University Press The Edinburgh Building, Cambridge CB2 2RU, UK Published in the United States of America by Cambridge University Press, New York www.cambridge. org Information on this title: www.cambridge.org/9780521473897 © Cambridge University Press 1998 This book is in copyright. Subject to statutory exception and to the provisions of relevant collective licensing agreements, no reproduction of any part may take place without the written permission of Cambridge University Press. First published 1998 This digitally printed first paperback version 2005 A catalogue recordfor this publication is available from the British Library Library of Congress Cataloguing in Publication data Abrate, Serge, 1953Impact on composite structures / Serge Abrate. p. cm. Includes bibliographical references and index. ISBN 0-521-47389-6 (he) 1. Composite materials - Impact testing. 2. Composite materials - Mechanical properties. I. Title. TA418.9.C6A25 1998 624.1'89-dc21 97-16551 CIP ISBN-13 978-0-521-47389-7 hardback ISBN-10 0-521-47389-6 hardback ISBN-13 978-0-521-01832-6 paperback ISBN-10 0-521-01832-3 paperback

Contents

Preface 1 Introduction 2 Contact Laws 2.1 Introduction 2.2 Contact between Two Isotropic Elastic Solids 2.3 Indentation of Beams 2.4 Indentation of Plates 2.5 Indentation of a Laminate 2.6 Elastoplastic Models 2.7 Conclusion 2.8 Exercise Problems 3 Impact Dynamics 3.1 Introduction 3.2 Beam Theories 3.2.1 Bending of a Beam by a Uniform Load 3.2.2 Higher-Order Beam Theory 3.2.3 Timoshenko Beam Theory 3.2.4 Bernoulli-Euler Beam Theory 3.2.5 Static Loading on Beams 3.2.6 Recovery of Accurate Stresses from Beam Models 3.2.7 Harmonic Wave Propagation 3.2.8 Free Vibrations of Beams 3.2.9 Effect of Geometrical Nonlinearities 3.2.10 Summary 3.2.11 Exercise Problems 3.3 Plate Theories 3.3.1 First-Order Shear Deformation Theory 3.3.2 Classical Plate Theory (CPT)

ix 1 6 6 7 9 13 15 19 24 24 26 26 27 27 29 31 32 32 35 36 39 44 46 47 48 48 54

vi

Contents

3.3.3 Higher-Order Plate Theory (HOPT) 3.3.4 Static Deflections of Plates 3.3.5 Harmonic Wave Propagation 3.3.6 Free Vibrations of Plates 3.3.7 Transient Response of a Plate 3.3.8 Variational Models 3.3.9 Effect of Boundary Conditions 3.3.10 Summary 3.3.11 Exercise Problems 3.4 Impact Models 3.4.1 Spring-Mass Models 3.4.2 Energy Balance Models 3.4.3 Response of Bernoulli-Euler Beam to Impact by a Mass 3.4.4 Impact on a Simply Supported Plate (Classical Plate Theory) 3.4.5 Impact on a Simply Supported Plate (SDPT) 3.4.6 Approximate Solution for Wave-Controlled Impacts 3.4.7 Summary 3.4.8 Exercise Problems 3.5 Theory of Shells 3.5.1 Equations of Motion 3.5.2 Simply Supported Panels 3.5.3 Exercise Problems 3.6 Scaling 4 Low-Velocity Impact Damage 4.1 Impact Tests 4.2 Failure Modes in Low-Velocity Impact Damage 4.2.1 Morphology of Low-Velocity Impact Damage 4.2.2 Damage Development 4.2.3 Qualitative Models for Predicting Delamination Patterns 4.3 Experimental Methods for Damage Assessment 4.3.1 Nondestructive Techniques 4.3.2 Destructive Techniques 4.3.3 Observation of Damage Development during Impact 4.4 Parameters Affecting Impact Damage 4.4.1 Material Properties 4.4.2 Target Stiffness 4.4.3 Projectile Characteristics

55 59 63 70 71 75 79 82 82 83 83 86 89 96 99 113 126 127 128 128 131 132 132 135 136 140 140 144 145 148 148 150 151 151 152 154 154

Contents

5

6

7

8

4.4.4 Layup and Stitching 4.4.5 Preload 4.4.6 Environmental Conditions 4.5 Summary 4.6 Review Questions Damage Prediction 5.1 Introduction 5.2 Damage in Thick Laminates 5.3 Damage in Thin Laminates 5.4 Damage Initiation 5.5 Propagation of Delaminations during Impact 5.6 Conclusion 5.7 Exercises Residual Properties 6.1 Introduction 6.2 Compressive Strength 6.2.1 Test Procedures 6.2.2 Experimental Results 6.2.3 Prediction of Residual Compressive Strength 6.3 Buckling 6.3.1 Thin-Film Delaminations 6.3.2 Delaminated Beam-Plates 6.3.3 Buckling of Beam-Plates with Multiple Delaminations 6.3.4 Buckling of Delaminated Plates 6.4 Residual Tensile Strength 6.4.1 Experimental Results 6.4.2 Prediction of Residual Tensile Strength 6.5 Residual Flexural Strength 6.6 Fatigue 6.7 Effect of Impact Damage on Structural Dynamics Behavior 6.8 Exercise Problems Ballistic Impact 7.1 Introduction 7.2 Experimental Technique s 7.3 Ballistic Limit and Residual Velocity of the Projectile 7.4 Failure Modes 7.5 Prediction of Ballistic Limit 7.6 Ceramic-Composite Armor Repairs 8.1 Introduction

vii 157 158 158 158 159 161 161 162 163 165 168 170 171 172 172 172 173 177 185 186 189 190 193 195 198 199 201 205 206 209 213 215 215 216 217 219 220 224 228 228

viii

Contents

8.2 Mechanically Fastened Patches 8.3 Adhesive Bonded Joints 8.3.1 Peel and Shear Stresses in a Double-Lap Joint 8.3.2 Bonded Metal Patch Repair 8.3.3 Bonded Composite Repair 8.3.4 Staggered Bonded Repair 8.3.5 Repair of Composite Sandwich Structures 8.3.6 Resin Injection 8.4 Repair of Thermoplastic Composites 9 Impact on Sandwich Structures 9.1 Introduction 9.2 Contact Laws 9.2.1 Compressive Behavior of Core Materials 9.2.2 Contact between a Sandwich Beam and a Cylindrical Indentor 9.2.3 Contact between a Sandwich Plate and a Spherical Indentor 9.3 Impact Dynamics 9.4 Impact Damage 9.4.1 Failure Modes 9.4.2 Governing Parameters 9.4.3 Improved Sandwich Construction 9.4.4 High-Velocity Impacts 9.5 Residual Properties References Index

230 231 232 235 236 236 237 237 238 240 240 240 241 245 247 248 249 249 251 254 255 255 258 287

Preface

As composite materials are used more extensively, a constant source of concern is the effect of foreign objects impacts. Such impacts can reasonably be expected during the life of the structure and can result in internal damage that is often difficult to detect and can cause severe reductions in the strength and stability of the structure. This concern provided the motivation for intense research resulting in hundreds of journal and conference articles. Important advances have been made, and many aspects of the problem have been investigated. One would need to study a voluminous literature in order to get an appreciation for this new research area. After writing three comprehensive literature reviews on the topic of impact on composite materials, I felt that there was a need to present this material in book form. The study of impact on composite structures involves many different topics, including contact mechanics, structural dynamics, strength, stability, fatigue, damage mechanics, and micromechanics. Impacts are simple events with many complicated effects, and what appears as a logical conclusion in one situation seems to be completely reversed in another. This variety and complexity have kept me interested in this area for several years, and I hope to communicate that to the readers. This book attempts to present this new body of knowledge in a unified, detailed, and comprehensive manner. It assumes only a basic knowledge of solid mechanics and the mechanics of composite materials and can be used as a text for a graduate-level course or for self-study. Exercise problems are proposed in order to challenge the user's understanding of the material. It is hoped that, after each section, the reader will gain an appreciation of the problems being addressed and the methods available and will be able to implement some of these methods. For example, after Chapter 3, "Impact Dynamics," the reader should understand what is involved in the selection of a mathematical model for predicting the contact force history and should be able to implement what appears to be the logical choice for the particular problem being considered. IX

x

Preface

Researchers and practitioners in industry would appreciate this comprehensive presentation of the state of the art in this area and use this book as a reference. A long list of references is included for those interested in more details. Current knowledge in certain areas has reached a certain level of maturity. For example, there is a general agreement on how to model the local indentation of a composite plate by smooth indentors. In other areas, current methods are not completely satisfactory, particularly in the areas of damage prediction and the prediction of the residual properties of impact-damaged composites. The book covers both low-velocity and ballistic impacts. Hypervelocity impacts encountered when spacecraft are hit by meteorites or space debris are in a different class, where impact velocities are measured in km/s. Too few studies dealing with this type of impacts on composite structures can be found, so this aspect of the problem was omitted. Recently, a new area of research dealing with smart materials and smart structures has developed, and one of the objectives has been to use distributed sensors and actuators to monitor the health of the structure. Several attempts were made to determine if and where an impact occurred or to determine the location and size of impact damage. This type of study is beyond the scope of this book, because it would require discussing the modeling of such sensors and actuators, control methods, and identification procedures. However, the methods for modeling the impact dynamics and for modeling the behavior of damaged structures discussed in this book will be very useful for modeling such smart structures. Upon reading this book, it will be obvious that I am indebted to the numerous investigators who have contributed to the development of this body of knowledge. I have made an effort to include every significant development and to acknowledge the source. A book is usually a reflection of the author's choices regarding what needed to be included and what could be omitted. A balance must be struck between the desire to be clear and comprehensive and the risk of overburdening the reader. In this case, almost every chapter could have been expanded to full book length, making it sometimes difficult to choose. However, I hope readers will gain a sufficient understanding of each aspect of the problem that they will be able to pursue its study on their own. The extensive list of references and the several available literature surveys should be helpful in this regard. Finally, I would like to thank my editor, Florence Padgett, for being so supportive of me in this endeavor. My wife Jayne and my sons Denis and Marc deserve thanks for allowing me to devote much of my free time to this project. Special thanks to my parents, who encouraged me to pursue my dreams and helped me get the best education. I wish my father were still with us to see this book completed. He would have been very proud.

1 Introduction

During the life of a structure, impacts by foreign objects can be expected to occur during manufacturing, service, and maintenance operations. An example of in-service impact occurs during aircraft takeoffs and landings, when stones -and other small debris from the runway are propelled at high velocities by the tires. During the manufacturing process or during maintenance, tools can be dropped on the structure. In this case, impact velocities are small but the mass of the projectile is larger. Laminated composite structures are more susceptible to impact damage than a similar metallic structure. In composite structures, impacts create internal damage that often cannot be detected by visual inspection. This internal damage can cause severe reductions in strength and can grow under load. Therefore, the effects of foreign object impacts on composite structures must be understood, and proper measures should be taken in the design process to account for these expected events. Concerns about the effect of impacts on the performance of composite structures have been a factor in limiting the use of composite materials. For these reasons, the problem of impact has received considerable attention in the literature. The objective with this book is to present a comprehensive view of current knowledge on this very important topic. A first step in gaining some understanding of the problem is to develop mathematical models for predicting the force applied by the projectile on the structure during impact. In order to predict this contact force history, the model should account for the motion of the structure, the motion of the projectile, and the local deformations in the contact zone. A detailed description of the contact between the impactor and the structure during impact would be difficult to obtain and is not required as part of the impact dynamics analysis. Instead, what is needed is a contact law relating the contact force to the indentation, which is defined as the motion of the projectile relative to that of the target. With the material systems commonly used, strain rate effects are negligible such 1

2

1 Introduction

that static and dynamic contact laws are identical, and so statically determined contact laws can be used in the dynamics analysis. Many investigators analyzed the loading phase of the indentation process and predicted the contact law for beams and plates with various boundary conditions and several indentor shapes. The indentation process introduces damage and permanent deformations in the contact zone; as a result, the unloading curve differs from the loading curve. In many cases, multiple impacts occur and the reloading curve is again different. While some simple analyses of the unloading and reloading phases have been presented, a complete and accurate characterization of the contact law for a particular target-indentor combination can only be obtained experimentally. A set of equations are commonly used to describe the contact behavior between solid laminates and smooth indentors, with a small number of constants to be determined from experiments. Contact problems are discussed in Chapter 2. An important aspect of a model for predicting the impact dynamics is to accurately describe the dynamic behavior of the target. For some simple cases, the motion of the structure can be modeled by a simple spring-mass system or by assuming a quasi-static behavior and considering the balance of energy in the system. But in general, more sophisticated beam, plate, or shell theories are required to model the structure. Two- and three-dimensional elasticity models are also employed. For each particular case, a choice must be made between a number of theories developed to account for complicating factors such as transverse shear deformation and rotary inertia. In addition, one must select to use variational approximation methods or finite element methods if exact solutions are not available for the case at hand. In Chapter 3, several structural theories are presented and their accuracies are discussed, particularly in regard to the impact problem. Several examples of impact dynamics analyses are presented for impacts on beams, plates, and shells. Often tests cannot be performed on full scale prototypes, so small specimens must be used. In other cases, tests or analyses have been performed on two specimens of different sizes. Methods developed to scale results obtained from a small-scale model to a full-size prototype are discussed in Chapter 3. Different test apparatus are used to simulate various types of impact. Dropweight testers are used to simulate low-velocity impacts typical of the tool-drop problem, in which a large object falls onto the structure with low velocity. Airgun systems, in which a small projectile is propelled at high speeds, are used to simulate the type of impacts encountered during aircraft takeoffs and landings. Testing conditions should replicate the actual impacts the structure is designed to withstand, and so the choice of the proper test apparatus is important. Descriptions of several common types of impact testers are given in Chapter 4, where damage development, the morphology of impact damage,

1 Introduction

3

and experimental techniques for damage detection are also described. Impact damage consists of delaminations, matrix cracking, and fiber failure. Extensive experimental investigations have revealed definite patterns for the shape of the damage and its initiation and growth. It is generally accepted that during low-velocity impacts, damage is initiated by matrix cracks which create delaminations at interfaces between plies with different fiber orientations. For stiff structures, matrix cracks start on the impacted face of the specimen due to high contact stresses. Damage propagates downward by a succession of intra-ply cracks and interface delaminations to give what is called a pine tree pattern. For thin specimens, bending stresses cause matrix cracking in the lowest ply, and damage progresses from the nonimpacted face up toward the projectile giving a reverse pine tree appearance. Many studies demonstrated that no delaminations are induced at the interface between plies with the same fiber orientation. The delaminated area at an interface depends on the fiber orientations in the plies adjacent to that interface. Of the large number of experimental methods that have been developed for damage assessment, some result in the complete destruction of the specimen and others are nondestructive, but most methods are used to determine the state of damage after impact. A few methods can be used to monitor the development of damage during impact. Once the failure modes involved are known and methods to assess damage are available, the next task is to determine what the governing parameters are. The properties of the matrix, the reinforcing fibers, and the fiber-matrix interfaces affect impact resistance in several ways, along with effects of layup, thickness, size, boundary conditions, and the shape, mass, and velocity of the projectile. Techniques for improving both impact resistance and impact tolerance will also be discussed. The prediction of impact damage is a difficult task for which complete success may not be possible and is probably not necessary. A large number of matrix cracks and delaminations are created in the impact zone, and the introduction of each new crack creates a redistribution of stresses. Thus it is not realistic to attempt to track every detail of damage development during the dynamic analysis of the impact event. Some purely qualitative models explain the orientation and size of delaminations at the various interfaces through the thickness of the laminate. Other models predict the onset of delaminations by predicting the appearance of the first matrix crack. Models for estimating the final state of delaminations are available. Chapter 5 deals with models for predicting impact damage. Impact-induced delaminations result in drastic reductions in strength, stiffness, and stability of the laminate, which explains why impact is of such concern to the designers and users of composite structures and why such effort has been directed at understanding the problem. Reductions are particularly significant

4

1 Introduction

in compression, where the effect of delaminations is more readily visible. The extent of these reductions has been characterized experimentally, and several mathematical models are used to predict the residual strength, as discussed in Chapter 6. Chapter 7 deals with high-velocity impacts. Sometimes the expression "highvelocity impact" refers to impacts resulting in complete perforation of the target. However, it must be recognized that complete perforation can be achieved both under low-velocity impacts when overall deflections of the target are taking place and under high-velocity impacts when the deformations of the target are localized in a small region near the point of impact. Here, high-velocity impacts are defined so that the ratio between impact velocity and the velocity of compressive waves propagating through the thickness is larger than the maximum strain to failure in that direction. This implies that damage is introduced during the first few travels of the compressive wave through the thickness when overall plate motion is not yet established. The ballistic limit is defined as the initial velocity of the projectile that results in complete penetration of the target with zero residual velocity. For impact velocities above the ballistic limit, the residual velocity of the projectile is also of interest. General trends for ballistic impacts (including the effect of several important parameters) are known from experimental results, and models for predicting the ballistic limit are available. Another area to be discussed in this chapter is the design of composite armor, which usually involves using one layer of ceramic material to blunt or fragment the projectile and another layer of composite material to absorb the residual kinetic energy. Many repair procedures for composite structures with impact damage have been reported. In selecting a particular repair technique, several factors must be considered, including the severity of the damage, the loads to be sustained, and the equipment available at the location where the repair procedure will be performed. In some cases, a successful repair cannot be made and the part must be replaced. In other cases, only cosmetic repairs are needed. In yet other cases, either bolted repairs or bonded repairs are needed. Proper design of the repair patch, machining, surface preparation, prefabrication of patches, and bonding are important phases of a successful repair procedure. The basic problems and most promising approaches are reported in Chapter 8. In many applications, sandwich structures with laminated facings are used because of the well-known advantages of this type of construction. The facings are loaded primarily in tension or compression to resist bending while the core resists the shear stresses. As a result, sandwich structures achieve a great bending rigidity, but in the transverse direction the rigidity remains low. A low rigidity in the transverse direction results in a low contact stiffness and

1 Introduction

5

lower contact forces during impact. Contact laws for sandwich structures are completely different from those of monolithic laminates and are dominated by the deformation of the core. Usually cores are made out of honeycomb materials, foam, or balsa wood. All these materials are considered to be part of the family of cellular materials and have a similar stress-strain behavior when loaded in compression in the transverse direction. The choice of a particular material is based on considerations of performance, weight, and cost. Models for predicting the behavior of a sandwich panel under a smooth indentor are discussed in Chapter 9. Impact creates damage to the facings, the core, and the core-facing interfaces. The evolution of damage with impact energy and its effects on the residual properties of sandwich panels are also discussed in that chapter.

2 Contact Laws

2.1 Introduction Local deformations in the contact region must be accounted for in the analysis in order to accurately predict the contact force history. The indentation, defined as the difference between the displacement of the projectile and that of the back face of the laminate, can be of the same order as or larger than the overall displacement of the laminate. One could consider the projectile and the structure as two solids in contact and then analyze the impact problem as a dynamic contact problem. However, this approach is computationally expensive and cannot describe the effect of permanent deformation and local damage on the unloading process. The unloading part of the indentation process can be modeled only using experimentally determined contact laws. To predict the contact force history and the overall deformation of the target, a detailed model of the contact region is not necessary. A simple relationship between the contact force and the indentation, called the contact law, has been used by Timoshenko (1913) to study the impact of a beam by a steel sphere. This approach has been used extensively since then and is commonly used for the analysis of impact on composite materials. Although the impact event is a highly dynamic event in which many vibration modes of the target are excited, statically determined contact laws can be used in the impact dynamics analysis of low-velocity impacts because strain rate and wave propagation effects are negligible with commonly used material systems. Hunter (1957) calculated the energy lost by elastic waves during the impact of a sphere on an elastic half-space. The ratio between the energy lost in the half-space and the initial kinetic energy of the sphere is given by V rV5 . 1.04 ( (2.1) Therefore, the energy loss is negligible as long as the initial velocity of the

22 Contact between Two Isotropic Elastic Solids

1

sphere, V, is small compared with c = (E/p)1^2, the phase velocity of compressive elastic waves in the solid. In many cases, the contact area is small and the behavior is similar to that observed during the indentation of a half-space. The indentation is independent of the overall deflection of the structure. When the contact area becomes large, the overall deflection of the structure affects the pressure distribution under the indentor; this interaction must be accounted for accurately. This chapter presents the basic results from contact mechanics needed to model the indentation of composite materials during the impact by a foreign object. The objective of such models is the accurate prediction of the contact force history and the overall response of the structure. 2.2 Contact between Two Isotropic Elastic Solids Detailed accounts of the study of contact between two smooth elastic solid pioneered by Hertz are given in several books (Barber 1992, Gladwell 1980, Johnson 1985, Timoshenko and Goodier 1970). Essential results from Hertz theory of contact as given here without derivation. For two isotropic bodies of revolution (Fig. 2.1), contact occurs in a circular zone of radius a in which the normal pressure p varies as

where po is the maximum contact pressure at the center of the contact zone and r is the radial position of an arbitrary point in the contact zone (Fig. 2.2). Defining the parameters R and E as

Figure 2.1. Two bodies of revolution for Hertzian analysis of contact.

2 Contact Laws

Figure 2.2. Pressure distribution in the contact zone.

where R\ and R2 are the radii of curvature of the two bodies. The Young moduli and Poisson's ratios of the two bodies are E\,v\, and E2, V2, respectively. Without loss of generality, the subscript 1 is taken to denote properties of the indentor and subscript 2 identifies properties of the target. The radius of the contact zone a, the relative displacement a, and the maximum contact pressure are given by a=

31

a3 ~R P0 =

(2.5)

—

' 4E =

( 9P2 \ ] \16RE2)

3P

2 i /6/>£2\ \

2*a* ~ V

(2.6) (2.7)

The force indentation law is expressed as P =

(2.8)

where P is the contact force, a is the indentation, and the contact stiffness k is given by k — —F /? 2"

o Q\

Equation (2.8) is usually referred to as Hertz contact law or the Hertzian law of contact and is found to apply for a wide range of cases, even if all the assumptions made in the derivation of the theory are not satisfied. For example, (2.8) also applies for laminated composites, even though these are not homogeneous and isotropic materials. With composite materials, permanent deformations are introduced in the contact zone for relatively low force levels, but the material is assumed to remain linear elastic in the analysis. Matrix cracks, fiber fracture, and interply delaminations can be introduced in the contact zone, but overall the contact law follows (2.8).

2.3 Indentation of Beams

9

The experimental determination of the contact law usually involves the use of a displacement sensor which directly measures the displacement of the indentor relative to the back face of the specimen. The plot of the applied force versus the indentation measured in this way follows the general form given by (2.8). Least-squares fits of the experimental data usually show that the exponent of a in that equation is close to | , and k is close to the value given by (2.9). Some investigators present plots of the contact force versus the displacement of the indentor that show a significant discontinuity when delaminations are introduced. The displacement of the indentor is the sum of the indentation and the deflection of the structure. The observed discontinuity corresponds to the reduction in the apparent stiffness of the structure caused by the introduction of delaminations.

2.3 Indentation of Beams During the indentation of beams, local deformations are superposed onto the overall deflection of the beam. When the beam deflections are small, the interaction between the local indentation and the overall deflection of the beam is negligible. Therefore, the indentation law and the pressure distribution in the contact zone are the same as for the indentation of a half-space. However, for flexible beams under large indentors, the beam may wrap around the indentor, leading to significant changes in the normal pressure distribution. First, consider the bending of a Bernoulli-Euler beam and neglect local deformations. This simple analysis will provide some understanding of the physical behavior of a beam loaded by a large indentor. From the free body diagram of an infinitesimal beam element (Fig. 2.3), the equilibrium equations for a planar beam are + V=0, (2.10) +p = 0, ^ dx dx where V is the shear force, M is the bending moment, and p is the applied force per unit length. With the Bernoulli-Euler beam theory, plane sections are assumed to remain planar and perpendicular to the neutral axis of the beam.

M

V Figure 2.3. Free body diagram of beam element.

10

2 Contact Laws

Figure 2.4. Simply supported beam with concentrated force applied in center. The axial displacements are then related to the transverse displacement by «(,,,) = -z*^>. dx

(2.11)

and the axial strain is d2w TTdx2 The bending moment is related to the transverse displacement by M = -

oxxzdA = JA

JA

(2-12)

EexxzdA JA

"2»

--*-

a,3,

The bending moment distribution in a simply supported beam of length L subjected to a concentrated force applied in the center (Fig. 2.4) is given by

for x > 0. The curvature of the beam is given by the second derivative of the deflection. Using (2.13) and (2.14), the load required to bend the beam to a radius R equal to that of the indentor is found to be

/>=4§[,

(2.15)

which indicates that wrapping is more likely to occur for long flexible beams under a large impactor. As the load increases, the beam comes in contact with the indentor over a distance a (Fig. 2.5). In that region, the radius of curvature is constant and equal to the radius of the impactor. Equation (2.13) implies that the bending moment is also constant, and (2.10) indicates that the shear force is uniformly equal to zero and that the pressure under the impactor is also zero. The beam is then loaded by two concentrated forces of magnitude P/2 located at +a and —a. The distance a is such that the curvature of the beam at x = a is equal to the

2.3 Indentation of Beams

11

Table 2.1. Analytical studies of contact between a beam and a rigid indentor Boundary conditions Simply supported

Indentor shape

Material Isotropic

Cylindrical

Orthotropic

Cylindrical

Clamped-clamped

Isotropic

Cylindrical

Cantilever

Orthotropic Isotropic

Cylindrical Cylindrical

Orthotropic

Flat Cylindrical Flat

Reference Keer and Miller (1983b) Sankar and Sun (1983) Shankar(1987) Sankar (1989a,b) Keer and Ballarini (1983a) Sun and Sankar (1985) Keer and Miller (1983b) Sankar and Sun (1983) Keer and Ballarini (1983a) Keer and Silva (1970) Keer and Schonberg (1986a) Keer and Schonberg (1986a) Keer and Schonberg (1986b) Sankar (1989a) Keer and Schonberg (1986b)

Figure 2.5. Beam wrapping around the indentor.

curvature of the indentor. For a < x < L/2, the bending moment is given by (2.14), and using (2.13) we find

« = f-2fi

(2,6,

for values of P larger than that given by (2.15). The conclusion from this simple analysis is that, neglecting local deformations, as a concentrated contact force would produce radius of curvature smaller than the radius of the indentor, the beam is loaded by two forces separated by a distance 2a. When local deformations are included, the pressure distribution is expected to be such that the maximum pressure is reached close to the edge of the contact zone. Beam theory does not predict those local deformations, and various approaches have been used to address the problem (Table 2.1). These investigators used various methods to study the loading portion of the contact laws for either

12

2 Contact Laws

0

0

0.25

0.5

0.75

Nondimensional distance Figure 2.6. Pressure distribution under a cylindrical indentor in contact with a simply supported beam (p = 0, 0.2, 0.4, 0.6, 0.8). isotropic or orthotropic beams. Of particular interest in these studies is the pressure distribution in the contact zone. Sankar (1989a) gave results for simply supported beams of length / centrally loaded by a rigid cylindrical indentor of radius R. The nondimensional contact pressure is given by p = (1 - x2)hl

- )8(1 - Ax2)}

(2.17)

where x = x/c, with c being the radius of the contact zone. The nondimensional contact pressure is related to the actual pressure by P=

nbc

, .

(2.18)

with c = c/l,fi = 8.755c 4 , B = ^§f(///?) 3 and Dx = Ex/(l - v?2), £>2 = 2Z?2/(^i + ^2)- M a n ( i ^2 are the roots of the bi-quadratic equation SnA.4 - (25i2 + S66)k2 + S22 = 0.

(2.19)

The components of the compliance matrix of the material are defined as •311 =

— ,

S22=—,

£2

c .312 =

Vl2

- —

,

c ^66 =

* -—.

(2.20)

2.4 Indentation of Plates

13

For small values of the parameter p, the contact pressure follows a Hertzian distribution (Eq. 2.2), but as f$ increases, the pressure is distributed more towards the edge of the contact zone as predicted by the beam analysis as shown in Fig. 2.6. This discussion indicates that as the beam becomes more flexible, the pressure distribution under the indentor becomes significantly different than that between the same indentor and a half-space. While this phenomenon may not have a major effect on the contact law, it will significantly affect the stress distribution under the impactor and should be considered when attempting to predict impact damage. Many investigators have studied the contact between smooth indentors and beams with various support conditions (Table 2.1); the reader is referred to these studies for further details.

2.4 Indentation of Plates Similarly, several analytical studies of the contact between a smooth indentor and laminated plates have been published (see Table 2.2). Many times the plate was modeled as an homogeneous orthotropic plate, but in some of the latest studies, the laminate nature of the composite is considered to determine the effect of the stacking sequence and the material properties on the contact law. An analysis of the indentation of simply supported laminated plates under rigid spheres using three-dimensional elasticity theory (Wu and Yen 1994) indicates that the stacking sequence has little effect on the contact law confirming previous experimental results (Tan and Sun 1985, Yang and Sun 1982). The contact force is found to be roughly proportional to the transverse modulus of Table 2.2. Analytical studies of contact between a plate and a rigid indentor

Material

Indentor shape

Isotropic

Sphere

Essenburg(1962) Keer and Miller (1983c) Chen and Frederick (1993)

Transversely isotropic

Sphere

Sankar (1985a) Cairns and Lagace (1987)

Laminate

Sphere

Wuetal. (1993)

Laminate

Sphere

Wu and Yen (1994)

Laminate

Sphere

Suemasuetal. (1994)

Reference

2 Contact Laws

14

0

0.5

1

1.5

Indentation 10~4mm Figure 2.7. Contact law predicted by Wu et al. 1993. the composite and independent of the longitudinal modulus, which had been suggested earlier by Yang and Sun (1982) based on experimental observations. When the contact force is small, plate thickness has essentially no effect on the indentation law. The contact behavior is then essentially the same as that for the indentation of a half-space. For larger indentations, the contact area increases, significant deviations from Hertzian contact law are observed, and changes in pressure distribution are similar to those shown in Fig. 2.6. In that case, laminate thickness has a significant effect on the force-indentation behavior. Wu et al. (1993) studied the contact between a composite laminate and a cylindrical indentor and showed that as the contact force increases, the contact behavior changes from a small contact area stage to a large contact area stage. During the small contact area stage, the size of the contact zone increases slowly and almost linearly with the contact force. As the contact force increases above a critical value, the size of the contact zone increases dramatically, and the contact pressure distribution changes dramatically from an Hertzian-type distribution to a saddle-type distribution of the type shown in Fig. 2.6. This characterizes the beginning of the large contact area. In Fig. 2.7, the small contact area

2.5 Indentation of a Laminate

15

phase corresponds to the curve between the origin and point A. Beyond point A, the indentation actually decreases as the force keeps increasing because of this redistribution of contact pressure over a larger area. Wu and Shyu (1993) showed that the contact force for the onset of delamination is independent of indentor size and that indentation consists of two stages. In the small indentation stage, the plate is still intact and the stacking sequence has insignificant effect on the force-indentation relationship. For large loads, damage becomes important, and the force-indentor movement curves differ for different layups. The contact behavior during low-velocity impacts is the same as in static tests.

2.5 Indentation of a Laminate A more practical approach consists of determining the relationship between the contact force and the indentation experimentally. Sun and coworkers (DanJumbo et al. 1989, Gu and Sun 1987, Sun et al. 1993, Tan and Sun 1985, Yang -and Sun 1982) studied the static indentation of laminated composites. Typically, during impact the contact force increases to maximum value and then decreases back to zero. In some cases, multiple impacts and reloading occurs. Therefore, contact laws should include the unloading and reloading phases. During the first loading phase, the contact law closely follows Hertz's law of contact (2.8). The parameter n in that equation is usually determined experimentally, but it can also be estimated if the radius of the indentor and the elastic properties of the impactor and the target are known using (2.9), with R given by (2.3). E in (2.9) is given by (2.4), Ei being the transverse modulus of the composite. Poisson's ratio of the composite is often taken to be zero (Yang and Sun 1982) in (2.4). Equation (2.8) describes the contact law during the loading phase of the indentation process. However, permanent indentation occurs even at relatively low loading levels, and the unloading phase of the process is significantly different from the loading phase. This phenomenon was observed by Crook (1952) for the indentation of steel plates by spherical indentors. During the unloading phase, the contact law suggested by Crook is P = Pm[(a - ao)/(am - ao)]2\

(2.21)

where Pm is the maximum force reached before unloading, am is the maximum indentation, and a0 is the permanent indentation. ao is zero when the maximum indentation remains below a critical value acr. When am > acr, ao = am[l-(acr/am)i].

(2.22)

16

2 Contact Laws

During subsequent reloading, the reloading curve is distinct from the unloading curve but always returns to the point where unloading began (Yang and Sun 1982). The unloading curve is modeled by P = Pm[(a - ao)/(am - ao)]l

(2.23)

The parameter ao does not necessarily correspond to the permanent indentation of the laminate, even though (2.23) indicates that P = 0 when a = a0, ao is selected so that (2.23)fitsthe experimental unloading curve using a least squares fit procedure. The parameter <x0 is related to the actual permanent indentation ap and the maximum indentation am during the loading phase by ao = P(am-ap)

(2.24)

when am > a cr ; G?O = 0 otherwise. The permanent indentation ap and the parameter ft are determined from experiments. However, many experiments need to be performed in order to determine these parameters, whereas a single unloading curve is necessary to determine acr when (2.22) is used. Yang and Sun (1982) presented experimental results for glass-epoxy and graphite-epoxy laminates. The elastic properties of the glass-epoxy material system were Ei = 39.3 GPa,

E2 = 8.27 GPa,

Gl2 = 4.14 GPa,

v12 = 0.26. (2.25)

For the loading phase, the contact law follows (2.8); for a 6.35-mm-radius indentor, the experimentally determined contact law is />exp = 1.60 x 10 4 c^,

(2.26)

and the predicted contact law is />pred = 1.90x lO 4 *!.

(2.27)

The critical indentation is 0.1016 mm (.004 in.). Figure 2.8 shows the loading curve given by (2.26) up to a maximum indentation of 0.3 mm and the corresponding unloading curve obtained from (2.21) and (2.22). If the indentation remains under 0.1016 mm, the unloading curve is identical to the loading curve, and as the maximum indentation becomes larger, the difference between loading and unloading paths is more pronounced. The area under the loading curve is the energy used to indent the laminate and is given by

U = ^JfcaL.

(2.28)

The area under the unloading curve is the energy recovered during the unloading

2.5 Indentation of a Laminate

17

3,000

2,500

2,000

1,500O LL 1,000-

500

0

i

0.05

0.1

i

0.15

I

0.2

r

0.25

0.3

Indentation (mm) Figure 2.8. Indentation of glass-epoxy laminate from Yang and Sum (1982). (a) Loading; (b) unloading; (c) reloading. process and is calculated using 2 7J

~

(2.29)

Cto)

For the case shown in Fig. 2.8, the ratio U'/U = 0.463 indicates that only 46.3% of the energy stored during the indentation process is recovered during unloading. This explains why, during the impact of a rigid structure where most of the impact energy is used for local indentation, the loading and unloading parts of the contact force history are significantly different. The reloading curve given by (2.23) is also shown in Fig. 2.8. After a first loading and unloading cycle, the target appears to be stiffer. Tests conducted on graphite-epoxy specimens with elastic properties Ei = 120.7 GPa,

E2 = 7.93 GPa,

Gn = 5.52 GPa,

v12 = 0.30 (2.30)

showed that the critical indentation was 0.0803 mm (3.16 x 10~3 in.).

2 Contact Laws

18

80

120

160

Maximum force (kN) Figure 2.9. Permanent indentation versus maximum contact force for the Kevlar-epoxy laminate tested by Meyer (1988). Meyer (1988) tested Kevlar-epoxy laminates with elastic properties Ex = 35.4 GPa,

E2 = 22.0 GPa,

vn = 0.175,

Gn = 7.36 GPa. (2.31)

A 15 cm x 15 cm x 2 cm piece cut from a cylindrical missile motor case with a 92.2 cm radius was continuously supported by a 92.2 cm steel platen and indented by a 25.4-mm-radius spherical indentor. The loading portion of the contact law is modelled by the equation P = 26 x l O V 2 5 .

(2.32)

During the unloading phase the behavior is modeled by

P=

Pm[{a-ao)/(ctm-ao)f

(2.33)

where the permanent indentation ao was shown to increase with the maximum load Pm (Fig. 2.9), and the exponent q has an average value of 4.1. It must be noted that the exponent in (2.32) is 2.25, compared to 1.5 for Hertzian contact,

2.6 Elastoplastic Models

19

Table 2.3. Experimental studies of contact Sun (1977) Lin and Lee (1990a) Leeetal. (1989) Meyer (1988) Sunetal. (1993) Cairns (1991) Swanson and Rezaee (1990) Wu and Shyu (1993) Yang and Sun (1982) Tan and Sun (1985) Dan-Jumbo et al. (1989) and that q = 4.1 for this Kevlar-epoxy laminate whereas for glass-epoxy and graphite epoxy the usual value is 2.5. The contact laws presented in this section are used extensively in the dynamic analysis of the impact event. Further experimental studies of contact can be found in the references listed in Table 2.3. 2.6 Elastoplastic Models With composites, permanent deformations are introduced when the indentation exceeds a small critical value. The material behavior in the transverse direction is governed by the properties of the matrix, and plastic behavior can be expected. Several investigators presented simple analyses for the indentation of a thin layer bonded to a rigid substrate (Cairns 1991, Christoforou 1993, Christoforou and Yigit 1994, Conway et al. 1970). First, the material is assumed to behave elastically until a critical indentation is reached. Then, the contact area is divided into a plastic zone and an elastic zone as the loading increases and a new contact law is obtained. Consider a laminate of thickness h, supported by a rigid substrate and indented by a rigid sphere of radius Rt (Fig. 2.10). The indentation is assumed to occur as if the material immediately under the indentor was subjected to uniaxial compression in the z-direction and the deformation takes place as shown in Fig. 2.10a. From that figure, the indentation a can be written in terms of the radius of the sphere, R(, and the contact radius, Rc, as a = Ri-(Rf-Rl)*.

(2.34)

The contact radius can be expressed as Rc = (2aRt -a2)1*.

(2.35)

20

2 Contact Laws

(b)

Figure 2.10. Indentation of thin layer supported by arigidsubstrate. In general, the indentation is much smaller than the radius of the indentor; considering the simplification made in this analysis, the second term on the right-hand side of (2.35) is neglected, yielding i.

(2.36)

The displacements under the indentor can be written directly from Fig. 2.10b as 8(r) =a-

R(

(2.37)

For small indentations, the contact radius is much smaller than the radius of the indentor, and the bracketed quantity can be simplified so that a-^-.

(2.38)

The transverse normal strain is assumed to as uniform through the thickness and is given by ezz = 8(r)/h. Assuming that the material behaves elastically, the contact force is given by P =

r

8(r)rdr,

(2.39)

2.6 Elastoplastic Models

21

Strain Figure 2.11. Stress-strain relations for elastoplastic analysis. where E is the modulus of elasticity in the transverse direction. Using (2.36) and (2.38), Eq. (2.39) gives the contact law (2.40)

for elastic contact. The model indicates that the contact force increases with a2 instead of a3/2, as predicted by Hertz law of contact. Permanent indentations are observed even for low values of the contact force. To account for these effects, assume that in the transverse direction the stressstrain behavior of the composite material is elastoplastic (Fig. 2.11). Because deformations are larger at the center of the contact zone, stresses will reach the yield strength first in the center, and the contact area can be divided into a plastic zone of radius Rp and an elastic zone between Rp and Rc. At the junction between the two zones, the stress is equal to the strength of material Zc so that Zc = j

(2.41)

Using (2.38), we find the radius of the plastic zone as (2.42)

as long as the indentation a is larger than the critical indentation Zch

acr. During the unloading phase, it is assumed that for r < Rp, the material will follow the elastic unloading path shown in Fig. 2.11 and that the stress-strain relation is given by cr = Zc + E(€-em). (2.46) The contact force during the unloading phase is given by P = 7tRiZc with Rp = [2Rt(am - Zch/E)]l/2.

After integration, (2.47) gives the contact

2.6 Elastoplastic Models

23

0 0

0.5

1

Indentation (mm) Figure 2.13. Comparison of experimental results with predictions of elastoplastic analysis (Eqs. 2.40, 2.45, 2.48). law for unloading TtRiE

(2.48)

for a > oio, with the permanent indentation ao defined as (2.49) Swanson and Rezaee (1990) conducted indentation tests on carbon-epoxy [0,±68,0]s laminates supported by rigid platen. The elastic properties of the material are Ex = 169 GPa,

E2 = 6.72 GPa,

v12 = 0.266,

Gn = 5.26 GPa, (2.50)

the thickness of the laminate is 2.4 mm, and the diameter of the indentor is 15.88 mm. The Hertz law of contact can adequately model the loading phase but for large loads (above 36,000 N), contact laws deviate significantly from Hertz law during the loading part of the indentation process. That smooth deviation is attributed to severe damage introduced during indentation of specimens that are back-supported by a hardened steel block. Figure 2.12 indicates that for

24

2 Contact Laws

these load levels the indentor has penetrated more than half the thickness. The elastoplastic analysis also provides a reasonable fit to the experimental data as shown in Fig. 2.13. 2.7 Conclusion It is generally accepted that for most current material systems such as graphiteepoxy or glass-epoxy, the indentation of a composite structure can be modeled using a statically determined contact law. The loading, unloading, and reloading portions of the force-indentation curves are modeled using (2.8), (2.21)-(2.23) with parameters usually obtained from experiments. Various aspects of the contact problem have been examined in details both experimentally then analytically, but these equations are now used by most investigators in mathematical models for the analysis of the impact dynamics.

2.8 Exercise Problems 2.1

Plot the loading phase of the contact laws for glass-epoxy, graphite-epoxy, and Kevlar-epoxy laminates under a 10-mm-radius indentor as the contact force increases from 0 to 1000 N. The material properties for these materials are given by (2.25), (2.30), and (2.31), respectively. 2.2 For the three materials in problem 2.1, plot the size of the contact zone and the maximum contact pressure as a function of the contact force. Discuss implications for stress distribution in the contact zone. 2.3 Starting with the Hertzian contact law, derive an expression for the energy required to produce a maximum indentation a max . What would be the energy needed if the contact force increases linearly to the same maximum level? 2.4 Consider a simply supported rectangular steel beam indented by a steel sphere. The indentation is expected to follow the Hertz law of contact. Find the overall deflection of the beam and the local indentation, and discuss the relative magnitude of these two deformations. When is one negligible compare to the other? 2.5 When unloading is governed by (2.21), derive an expression for the energy recovered during the unloading process. 2.6 Many investigators neglect local indentation altogether, and others assume that both the loading and the unloading phases are governed by Hertz law and obtain excellent agreement with experimental results. Discuss when local indentation effects can be neglected and when they must be considered, and to what extent.

2.8 Exercise Problems 2.7

25

Thermoplastic composites are known to be more damage resistant. Explain how a lower transverse modulus would affect the contact stiffness, the size of the contact area, the pressure distribution under the indentor, and therefore impact resistance.

3 Impact Dynamics

3.1 Introduction A first step in gaining some understanding of the effect of impact by a foreign object on a structure is to predict the structure's dynamic response to such an impact. Predictions are made using a mathematical model that appropriately accounts for the motion of the projectile, the overall motion of the target, and the local deformations in the area surrounding the impact point. In general, details of the local interaction between the projectile and the target are not needed to predict the contact force history. A particular beam, plate, or shell theory is selected, and the local deformation in the through-the-thickness direction, which is not accounted for in such theories, is included through the use of an appropriate contact law. Contact laws relate the contact force to the indentation, which is the difference between the displacement of the projectile and the displacement of the target at the point of impact. With most low-velocity impacts, small amounts of damage are introduced in a small zone surrounding the impact point, and the dynamic properties of the structures usually are not affected by the presence of damage. Therefore, impact dynamic analyses generally do not attempt to model damage as it develops during the impact event. The choice of a particular structural theory must be based on careful consideration of the effect of complicating factors such as transverse shear deformation and rotary inertia. For example, for beams, one can select to use the BernoulliEuler beam theory, the Timoshenko beam theory, or one of several other available beam theories. Similar choices are available for plates and shells, and the structure also can be modeled as a two- or three-dimensional solid. In this chapter, we will first present brief derivations of several beam, plate, and shell theories outlining the basic assumptions. Results from these different models are compared using static loading examples, free vibration examples, and wave propagation examples.

26

3.2 Beam Theories

27

Exact solutions to the equations of motion are available for some special cases of beams, plates, and shells subjected to dynamic loading. These solutions can be used effectively, but generally, approximate solutions must be sought. The finite element method is used often because it can be readily applied to a wide range of geometries and boundary conditions. Variational approximation methods are also used since in some cases they can provide more efficient solutions. The implementation of such methods, particularly with reference to the impact problem, is also discussed at length. To reduce cost, often tests are performed on small specimens rather than on full-scale prototypes. Whether such a scaling is possible and how to relate the results obtained on a small-scale model to the expected results on a full-scale model are also discussed in this chapter. 3.2 Beam Theories In this section we present the basic assumptions and the development of three beam theories: a higher-order theory, the Timoshenko beam theory, and the Bernoulli-Euler beam theory. Results from these theories for static loading, free vibration, and wave propagation examples will be compared in order to determine the applicability of each theory. 3.2.1 Bending of a Beam by a Uniform Load The following example, treated as a two-dimensional elasticity problem without any assumptions for a particular beam theory, is discussed to bring some understanding about the general behavior of beams, insight into why some of the assumptions in the various beam theories are made, and an understanding of each theory's limitations. Consider an isotropic beam of narrow rectangular cross section supported at the ends and subjected to a uniformly distributed load q (see Fig. 3.1). For this two-dimensional problem, the theory of elasticity (Timoshenko and Goodier 1970, pp. 46-48) indicates that the three nonzero stress components are 2/ V3~

2/

10*7

21*"

~

""" '

(3 la)

'

3 Impact Dynamics

28

Z

TTTTTTTT q

Figure 3.1. Simply supported beam subjected to uniform loading. where / is the moment of inertia of the beam. Equation (3.1c) indicates that the transverse shear stress axz follows a parabolic distribution through-thethickness of the laminate. The first term in (3.1a) represents the linear distribution through-the-thickness of the normal stress oxx that is predicted by the elementary beam theory. The second term in (3.1a) is the correction due the effect of the transverse normal stress azz, given by (3.1b). The normal stress axx reaches a maximum at x = 0 and z = h/2, at that point the second term in (3.1a) is less than 1% of the first term when L/ h > 2.58. Therefore, for most beams this correction term can be neglected, and the elementary beam theory is sufficiently accurate for most applications. In addition (3.1b) indicates that the transverse normal stress ozz is independent of x and has a maximum value of q at the bottom of the beam. The maximum value of ozz is less than 1% of the maximum value of oxx when L/h > 5.8. Therefore, for most beams this stress component is very small, its contribution to the total strain energy is small, and its effects are neglected in most beam theories. From two-dimensional elasticity, the displacements at an arbitrary location are u = 2EI h2

(3.2a)

v = —- 2EI h2x2 2EI

~2

12

(3.2b)

where u is the axial displacement; v is the transverse displacement; and 8 is the

3.2 Beam Theories

29

transverse displacement of the center of the beam (x = z = 0), which is given by 5 qLA where v is the Poisson's ratio for the material. The factor before the brackets in (3.3) is the deflection predicted by the elementary beam theory, and the second term inside the bracket represents the effect of shear deformation. As the ratio L/h becomes large, the effect of shear deformation becomes small. For a typical value of v = 0.3, this correction factor is less than 0.01 when L/h > 15. Therefore, for long beams the effect of shear deformations can be neglected as in the elementary beam theory. In the beam theories to be discussed here, the transverse normal strain is neglected, and the three theories differ in the way shear deformation is accounted for. With the higher-order theory, the transverse shear strain is assumed to follow a parabolic distribution and vanish on the top and bottom surfaces, as suggested by (3.1c). With the Timoshenko beam theory, the transverse shear strain is assumed to be constant through-the-thickness; with the Bernoulli-Euler beam theory (also called the elementary beam theory), the effect of transverse shear deformation is ignored altogether. 3.2.2 Higher-Order Beam Theory The development of the present higher-order beam theory is based on two hypotheses: (HI) The transverse shear strain vanishes on the top and bottom surfaces and follows a parabolic distribution through-the-thickness. (H2) The transverse normal strain can be neglected. These two hypotheses can be expressed as du dw ( 4z2\ ^z = 7 - + T - = y l - T T

.... ( 3 - 4a )

dw ezz = — =0 (3.4b) dz where y is the magnitude of the shear stress along the jc-axis. Equation (3.4b) yields w = wo(x), (3.5) and, after substitution into (3.4a), the axial displacement can be expressed as 4z3 u = uo(x) + z(y - wo,x) - — y.

(3.6)

30

3 Impact Dynamics

Considering only bending deformations (uo(x) — 0), and introducing the new variable \/r = y — wOiX, we obtain u = z^-^(f

+ wo,x).

(3.7)

From this equation, a physical interpretation of the function *I> is that it represents the rotation of a small line segment initially perpendicular to the jc-axis at z = 0. Equations (3.5) and (3.7) are the kinematic assumptions of the theory from which we get the two nonzero strain components du 4z3 txx = — = Zty, x - X77(V' + ™o,x),x dx 3hz

z2\

(

}

The strain energy, kinetic energy, and potential energy of the external forces are given by

U = \ [ (axxexx + 25. So far, this example indicates that shear deformations have a significant effect on the deflections for short beams and that this effect is more pronounced for composite beams. Now let us compare the stress distributions predicted by the beam theories with the elasticity solution. With the Bernoulli-Euler model, substituting (3.22) into (3.19b) and using Hooke's law, the axial stress is CTrx

=

(3.27)

3.2 Beam Theories

35

which is just the first term in (3.1a). The Timoshenko beam theory yields the same expression for the axial stress (3.27) and the following expression for the transverse shear stress: axz = —±-x. KA

(3.28)

With the higher-order theory, the transverse shear stress is

which is, for a rectangular beam, the exact result from the theory of elasticity. This indicates that the higher-order beam theory gives a much better prediction of the transverse shear stresses. The drawback is that the corresponding equations of motion and the boundary conditions are more complex than with the other theories. 3.2.6 Recovery of Accurate Stresses from Beam Models If an accurate determination of the transverse shear stresses is needed, it is possible to use the simpler elementary beam theory to determine the axial stress and then to use this result to determine the shear stresses from the equations of equilibrium of two-dimensional elasticity. For example, with the simply supported beam under uniform loading, the axial stress is accurately predicted (3.27) by the Bernoulli-Euler beam theory. Considering the beam as a two-dimensional solid, in the absence of body forces, equilibrium in the x-direction is governed by ^ I + ^i=0. ax dz From (3.30), the shear stress at location z is given by °zx X,Z - J

(3.30)

(3.31)

Substituting the expression for axx obtained from the Bernoulli-Euler beam theory (3.27), we find

which is precisely the exact solution for a rectangular beam obtained from the theory of elasticity (3.1c). Similarly, from two-dimensional elasticity, the equation of equilibrium in the z-direction is ^ + ^ = 0 . dx dz

(3.33)

36

3 Impact Dynamics

Integrating through-the-thickness from the bottom of the beam to an arbitrary location z, we obtain (J«(JC,

z)+q = - I' J_|

dGxz{ Z

^ ^dz\ dx

(3.34)

Substituting the value of the shear stress given by (3.32), the exact value of the transverse normal stress given by (3.1c) is recovered from (3.34). Therefore, it is possible to accurately determine both the transverse normal stress and the transverse shear stress distributions from the results of the elementary beam theory. 3.2.7 Harmonic Wave Propagation In order to compare the dynamic behavior of beams described by the three theories previously discussed, consider the propagation of free harmonic waves of the form w = We1"***-"0,

ir = W ^ - * 0

(3.35a,b)

where k is the wavenumber and co is the frequency. The wavenumber is related to the wavelength of the disturbance by k = In /A., and the phase velocity is c = co/k. Studying the propagation of free harmonic waves in an infinite beam allows us to gain some understanding about the dynamic behavior of the beam. Substituting w from (3.35a) into the equation of motion for a BernoulliEuler beam (3.20) gives co2 = ^jk4, or in terms of the phase velocity, c = (^j)l^2k. This indicates that beams are dispersive because the phase velocity depends on the wavelength, and that waves with shorter wavelengths propagate faster than waves with longer wavelengths. With this beam theory, however, short wavelengths can propagate with infinite speeds, which is not physically possible. This problem is the direct result of the simplifying assumptions made in the development of that theory. Substituting (3.35) into the equations of motion of a Timoshenko beam (3.16) gives the system of homogeneous equations:

K

» H-^[Ml1 2i

where A'n = KGAJC2, Mn = pA,

K22\

*]){W}=0

[M2l M22\)\V\

K22 = KGA + Elk2,

M22 = pi,

M

K12 = -K2\ = iicGAk,

M\2 = M2\ = 0.

(3.36) K } (3.37)

For nontrivial solutions, the determinant of the matrix of the coefficients in

3.2 Beam Theories

37

(3.36) must vanish, which gives the dispersion relation

pApIco4 - o)2[pA(EIk2 + KGA) + tcGApIk2] + tcGAEIk4 = 0.

(3.38)

This equation shows that for a given value of k there will be two solutions for the frequency or phase velocity. Plots of phase velocity versus wavenumbers are called dispersion curves, and in this case we will have two branches. For very long wavelengths, k approaches zero and (3.38) gives the two cutoff frequencies co\ = 0, o>i = (GA/pI)l/2. The first branch corresponds to bending motion, and the second branch to shear deformation. It can be shown that a first approximation to the first branch is co2 = ^jk4, which means that for long wavelengths the Timoshenko beam theory will predict the same behavior as the elementary beam theory. For short wavelengths (large values of k), Eq. (3.38) implies that the phase velocities tend to two limiting values: d = (icGA/pA)l/2,C2 = (El/pi)1/2. Therefore, the phase velocities are bounded for short wavelengths. The equations of motion of the Timoshenko beam can be written as uncoupled: EIwyXXXX + pAwjt - \pl + pA—— KGA\ [ EIf,xxxx

w,xxtt H

+ pAyjf,tt - \pl + pA—— 1, L KGA\

——Wjttt = 0

(3.39)

KGA tXXtt

+ £-A-^ KGA

=

o.

(3.40)

Abramovich and Elishakoff (1990) neglected the wJttt terms in these equations and obtained solutions to free and forced vibration problems. For free wave propagation, the effect of this simplification is to remove the pA pi co4 term from the dispersion equation (3.38). In that case, there is only one branch of the dispersion curve, and the phase velocity tends to the limit £ = (|y + ^ ) 1 / 2 for short wavelengths. After substituting (3.35) into the equations of motion for the higher-order beam theory (3.11), the dispersion relations are given by (3.36) with

K

a

" ' ^ ; ~ = pA H k ,

16 A/12 = —plki,

M

105

2X

(3.4.)

68

M22 =

pi,

= -MX2.

The two cutoff frequencies for long wavelengths are co\ =0,oo2 = (^^j)1^2. The shear correction factor K used in the Timoshenko beam theory is now

38

3 Impact Dynamics

100

200

300

400

Wavenumber k Figure 3.3. Dispersion curves for a steel beam with rectangular cross section. Solid line: Timoshenko's beam theory; dashed line: Bernoulli-Euler beam theory; dotted line: higher-order theory. replaced by | | = 0.8235 in the expression for the second cutoff frequency. In many cases, K is taken to be | = 0.8225 for beams with rectangular cross sections. For short wavelengths, the phase velocity tends to limit c = (EI/pI)l/2 for both modes. Example 3.1: Wave Propagation in Isotropic Beam To compare the three beam theories, consider the example of a steel beam with E = 210 GPa, v = 0.3, h = b = .05 m, p = 7850 kg/m3. For A: < 100, the higher-order theory and the Timoshenko beam theory give very similar results (Fig. 3.3). The higher-order theory will not bring about drastic changes in the predictions of the dynamic behavior of the beam. For the first mode, the phase velocity predicted by the Timoshenko beam has nearly reached its asymptotic value of 2928 m/s when k = 400, while with the higher-order theory the phase velocity keeps increasing to eventually reach a much higher asymptotic value of 5172 m/s. Figure 3.3 also shows the results obtained from the Bernoulli-Euler beam theory which

3.2 Beam Theories

39

indicate that this theory is applicable only for very long wavelengths k or small values of k{k = InIX). 3.2.8 Free Vibrations of Beams Another way to study the dynamics of the various beam theories is to study the free vibrations of finite beams. The natural frequencies of a simply supported beam of length L are identical to the frequencies of free harmonic waves with wavenumbers k = in/L. The study of harmonic wave propagation indicated that differences between the Timoshenko beam model and those from the higher-order theory are small. Therefore, the higher-order theory will not be considered in this section. Exact solutions for simple beams with any combination of boundary conditions at the ends will be developed for both the Bernoulli-Euler and the Timoshenko beam theories. An example of a clampedclamped beam will be used to illustrate the effect of the slendemess ratio, shear deformations and rotary inertia on the natural frequencies. For free vibrations of a Bernoulli-Euler beam, the displacements are taken in the form w(x, t) = W(x) sin(a)t).

(3.42)

Substituting (3.42) into the equation of motion (3.20) gives the ordinary differential equation dW El—- 4 dx

pAa)2W = 0.

(3.43)

Seeking a solution of the form W = e^*^, we find by direct substitution that (3.43) is satisfied for four distinct values of P*

ft = iP, fi = -iP, where fi = (co2pA/EI)l/4. form

P*3=P,

PZ = -P

(3.44)

This indicates that the general solution is of the

W(x) = A sin px + B cos fix + C sinh fix + D cosh

fix

(3.45)

where the constants A, B, C, and D have to be determined from the boundary conditions. Since there are two boundary conditions at each end of the beam, using (3.45), a system of four equations of the form

(3.46)

40

3 Impact Dynamics

will be obtained. For each of the natural frequencies of the beam, the determinant of the matrix K vanishes so that a nontrivial solution can be obtained for the four constants A-D. Therefore, the natural frequencies for beams with any combinations of natural frequencies at the ends can be determined by finding the zeroes of a 4 x 4 determinant. Exact solutions for the free vibration of Timoshenko beams are obtained by substituting w = WePx sin cot,

f = Xtfix sin cot

(3.47)

into the equations of motion (3.16), which leads to

Uf

+ pAa?)

GAP 2

[

- pico +

]]IW\-0 GA)\

)\ \ X J ~

a

Nontrivial solutions are obtained when the matrix of the coefficients vanishes, which implies that fi satisfies the bi-quadratic equation

^"4

GAEI

El

"2 °

^

This equation will have two solutions with the corresponding mode shapes

where 0 n = -GAjSi, 02i = —GAfc, The general solution is

0i2 = GApl + pAco2 , , 022 = GAfy + pAco .

W = A(pn sin^ix + Bcpn

(3-51)

COS^IJC

+ C(p2\ sinh p2x + C^2i cosh fax X = A2

El

-12 -6L 12

6L

(2 - 0)L2 -6L

(4 + 0)L

symmetric

(3.53)

2

where

0

12 / E I \ L 2 \KGA '

(3.54)

The mass matrix is the sum of two matrices: the matrix associated with translational inertia

[MpA] =

pAL

^22

^23

21O(l+0) 2

(3.55)

m34

symmetric

W44J

with

mu = m33 = 7O02 + 1470 + 78,

m12 = (3502 + 770 + 44)-,

4 mu = - ( 3 5 0 2 + 630 + 2 6 ) - , 4 (3.56) L2 L = m44 = {Icf)2 + 140 + 8) — , m23 = (350 2 + 630 + 2 6 ) L2 L 2 = - ( 7 0 + 140 + 6) — , m34 = - ( 3 5 0 2 + 770 + 4 4 ) - ,

mn = 350 2 + 630 + 27, m22 m24

and the matrix associated with rotatory inertia

[MpI] =

^22

3O(1+0) 2 L

^23

^24

m33

m34

(3.57)

symmetric m n ~~ ^13

==

^33 ~~ 36,

mi2 = mi4 = —^3

m22 = m44 = (1O02 + 50 + 4)L 2 , 2

4

==

—(150

— 3)Z^,

m23 = - ( 1 5 0 - 3)L,

(3.58)

2

m24 = (50 - 50 - 1)L . To ascertain the accuracy of that finite element, consider the error in the eigenvalues obtained using uniform meshes with increasing numbers of elements.

3.2 Beam Theories

43

The error is defined as (3.59) where the subscript / denotes the /th natural frequency and the superscript E indicates the exact value of the natural frequency or eigenvalue. Example 3.3: Convergence of Finite Element Analysis of Beam Vibrations The example treated by Friedman and Kosmatka (1993) is a simply supported beam with £7 = 1,

pA = l,

h/L = 0.2,

v = 0.3

(3.60)

with the shear correction factor 10(1 + v) K

=

Because of symmetry, only half of the beam needs to be modeled. Figure 3.5 shows that the error varies with h2, h being the length of one element-or 1E+00

1E-01

1E-02

1E-03

LJJ 1E-04-

1E-05-

1E-06 4

40

Number of elements Figure 3.5. Modelization error in finite element analysis of free vibration of beams.

44

3 Impact

Dynamics

Table 3.1. Natural frequencies of simply supported beam Mode

1 2 3 4 5 6

32 Elts.

Exact

Error

9.28200 32.24894 61.72164 93.81159 126.88143 160.26995

9.281920 32.24561 61.69867 93.73128 126.6825 159.8679

1.767e-5 2.066e-4 7.447e-4 1.714e-3 3.143e-3 5.036e-3

in other words, E varies with N 2, N being the number of elements in the discretization. As expected, the error increases for higher modes. Table 3.1 shows the accuracy of the first six natural frequencies obtained using a uniform mesh with 32 elements.

3.2.9 Effect of Geometrical Nonlinearities Since many composite structures are thin and flexible, moderately large deformations can be expected during impact. The effect of membrane stiffening on the impact dynamics and the contact force history should be investigated. Large displacements induce a coupling between axial and transverse displacements. For a Bernoulli-Euler beam, the kinematic assumption is written as u = uo —

(3.62)

zw;

where uo is the axial displacement and w is the transverse displacement. For moderately large displacements the axial strain is given by 1

l

-W

2 x.

(3.63)

When the material follows Hooke's law, the strain energy in the beam is given by

*xx}dx. +EIw*

(3.64)

The kinetic energy stored in the beam is given by T

= ? / [("« - z ^ * ) 2 + «£] dV = 1 / [PA(u2o + w2) + plw2x] dx. ^ JO

^ JO

(3.65) (365)

3.2 Beam Theories

45

Hamilton's principle (3.10) is used to derive the equations of motion l

(

i\

EA I uOjX + - w x I

= pA uo

f uo,x + -w2x )w,x\ ~ EIw,xxxx L\ ^ / J ,x and the boundary conditions where either EA

u

or

or

+ +

-EAluOjX or

= 0

w

-EIw,xx

(3.67) 1

- EA ( M

EIwxxx

(3.66a,b)

- pAw + pliv,xx

are prescribed at the ends. Since the effects of inplane inertia and rotary inertia are usually negligible, the right-hand side of (3.66a) and the pi term in (3.66b) are neglected, and the equations of motion now read = 0 x

EIwxxxx

+ pAih = EA

x

-,

(3.68a,b)

I uo,x + -w

Integrating (3.68a) gives *o,x + ^2X

= C{f).

(3.69)

w\dx.

(3.70)

Integrating again gives C(t) = ^-

f

After substitution into (3.68b), \ EA ( fL EIw,xxxx + pAib = —— I / w 2xdx w,xx. (3.71) lL \Jo ' / For simply supported beams, a one term Rayleigh-Ritz approximation can be obtained by taking w = a sin — . (3.72) Li

Substituting into (3.71), multiplying by sin ^ , integrating over the length of the beam, and using the change of variables r = cot, where a? = (f ) 4 ^ , yields the well-known Duffing equation: a + a + ea3 = 0

(3.73)

3 Impact Dynamics

46

— Exact --RR1

6-

4-

3

0

1

2

3

4

5

Amplitude / radius of gyration Figure 3.6. Effect of geometrical nonlinearities on the free vibrations of beams.

where _ A _ 1 (3.74) 4/ = 4 ^ and r is the radius of gyration of the cross section. Using the Linstedt-Poincare perturbation approach, the ratio of the nonlinear and linear fundamental frequencies is obtained as € =

coL

3 1 , 3 _2 = 1 + -€az = 1 + — 8 32 32

-\ 2

- I W

(3.75)

where a is the vibration amplitude. Figure 3.6 shows that when the amplitude remains small compared with the radius of gyration of the beam cross section, the nonlinear effects remain small and a linear model can be used. 3.2.10

Summary

Any beam theory is based on a set of assumptions aimed at reducing the threedimensional elasticity problem to a one-dimensional problem. In this section,

3.2 Beam Theories

47

we reviewed the basic assumptions made in the development of three basic theories: the Bernoulli-Euler beam theory, the Timoshenko beam theory, and a higher-order theory. The equations of motions and boundary conditions were derived from Hamilton's principle in a consistent way for each theory. The example of a simply supported beam subjected to a uniformly distributed load was used to compare the stresses and deflections predicted by the various beam theory to elasticity results. The objective was to evaluate the validity of the assumptions made in the development of the theories and to develop some general guidelines concerning the applicability of these theories. This example showed that for slender beams, the Bernoulli-Euler beam theory, which is the simplest of the three, provides very accurate results, but for shorter beams, the Timoshenko beam, which accounts for transverse shear deformations, is required. Shear deformation effects depend on the ratio of the elastic and shear moduli and therefore are more pronounced for composite beams, since the ratio is usually much higher for composites than for steel or aluminum. An analysis of harmonic wave propagation in beams shows that for most practical cases, the higher-order theory gives results that are very close to those predicted by the Timoshenko beam theory. Therefore, the increased complexity of the theory is not justified by any improvement in the results. Free vibration analyses show the importance of transverse shear deformation and rotary inertia on the dynamic behavior of beams. The effect of large deformations is investigated by considering the large-amplitude vibration of simply supported beams. Results show that as long as the amplitude remains small relative to the radius of gyration of the cross section, nonlinear effects are negligible. In many cases, impact tests are performed on beam specimens, and the beam theories discussed in this section will be used in the development of mathematical models for studying the impact dynamics. In addition, the knowledge about the various assumptions and the effects of shear deformations and rotary inertia gained through this study of beam theories will be directly applicable to the development of plate and shells theories examined in the following sections.

3.2.11 Exercise Problems 3.1

3.2

Using the Timoshenko beam theory, derive an expression for the static deflection of a cantilever subjected to a concentrated force P at the end. Show the effect of the slenderness h/L ratio on the magnitude of the shear deflection relative to the bending deflection. Following the approach shown Section 3.28, formulate the free vibration problem for a cantilever Bernoulli-Euler beam. Write down the four

48

3.3

3.4

3.5

3 Impact Dynamics boundary conditions in the form given by (3.46), and expand the 4 x 4 determinant to obtain the characteristic equation. Derive a beam theory neglecting the transverse normal strain and assuming that the transverse shear strain varies as a cosine function of z that vanishes on the top and bottom surfaces and reaches a maximum for z = 0. Determine the axial stresses and the transverse shear stresses in a simply supported, rectangular, Timoshenko beam subjected to a sinusoidally varying distributed load that vanishes at both ends. Compare with the results obtained using the Bernoulli-Euler beam theory and determine the effect of shear deformation. Use the approach shown in Section 3.2.6 to determine the transverse shear distribution from the results of the Bernoulli-Euler beam theory. Write a computer program to calculate the natural frequencies of Timoshenko beams using the exact approach discussed in Section 3.2.7. 3.3 Plate Theories

From the discussion on the effect of shear deformation and rotary inertia on the static and dynamic behavior of beams, it is expected that these two factors will have similar effects on the behavior of plates, particularly for plates made out of composite materials. The first-order shear deformation theory (FSDT), also known as the Mindlin or Mindlin-Reissner plate theory, which is an extension of the Timoshenko beam theory, will be presented first. For thin plates, the effect of shear deformation and rotatory inertia are small, and the theory can be reduced to the classical plate theory (CPT), which is the equivalent of the Bernoulli-Euler theory for beams. Higher-order plate theories are also available and will be discussed. 3.3,1 First-Order Shear Deformation Theory Following the discussion on beam theory, the development of a plate theory following the lines of the Timoshenko beam theory proceeds by assuming that the transverse normal strain ezz is negligible and that the two transverse shear strains are constant through-the-thickness. These two assumptions, which can be written as €zz = — =0 €xz

= ^ dv

(3.76a)

+ ^

= yi

dw

*yz = T - + - 7 - = K2,

oz

(3.76b)

oy

(3.76C)

3.3 Plate Theories

49

imply that the displacements are of the form u(x, y, z) = uo(x, y) + z(y\ ~ wo,x) v(x, y, z) = vo(x, y) + z(y2 - wOtX)

(3.77)

w(x,y,z) = wo(x,y). The change of variables

gives the displacement field of the first-order shear deformation theory in its usual form: u(x, y, z) — uo(x, y) + zirx(x, y) v(x, y, z) = vo(x, y) + zfy(x, y)

(3.79)

w(x,y,z) = wo(x,y) where uo,vo, wo are the displacement components of a point on the midplane. y\rx and \//y are the rotations of the normal to the midplane about the y- and ~;t-axes respectively. Equations (3.79) are often postulated as an assumption on the kinematics of the deformation in which a line segment initially normal to the midplane of the plate is assumed to remain straight but not necessarily normal to the midsurface during deformation. The infinitesimal strain components, defined as du dv dw yy zz dx' dy' dz ' (3.80) du dv du dw dv dw ^ y = 9y + a ? €xz = lh + 3Jc"' €yz ~ ~dz + ~dy' can be evaluated from (3.79): duo dx ezz = 0,

d\fsx dx ' exy =

duo

yy

1

dvo

dvo

d\/sy

dy

dy

h"

(dilfx

'

d\lr^

The plate is subjected to a distributed load q over the surface, normal inplane force resultants Nn over a part of the boundary T\,NS over F2, moment resultants Mn and Ms over F 3 and F 4 respectively, and transverse shear Qn forces over F5. The inplane force resultants are defined as (N;,Ny,Nxy)= = / J

(a(a ,oxy Xi,

•

o-0.20

^ •

\

x

•-

^k,,-

I

I

I

I

2

4

6

8

I

I

I

10 12 14 16

Radius/thickness Figure 3.14. Displacements of infinite plate subjected to a step load.

boundaries. After that time, the response will be affected by the boundary conditions. A solution for finite-sized composite plates is presented now to investigate the effect of finite size and anisotropy. The distributed loading and the displacement functions for a shear deformable plate (FSDT) can be expanded into the double Fourier series

E m,n=l

qmn(

mnx a

Wmn(t) sm

w = m,n=l oo

Xmn(t)cos m,n=\ oo

m7tx

sin mitx . nny

mnx

> sin

nny b

(3.191)

sin——

nny

cos ——.

In this way, for a simply supported plate with symmetric layup and no bendingtwisting coupling, the boundary conditions (3.139)-(3.140) are satisfied.

3.3 Plate Theories

75

Substituting (3.191) into the equations of motion (3.110)—(3.112) yields for each mode the set of three ordinary differential equations [M] I Xmn \ + [K] lxmn

\ = I 0 V

[ Ym J

Ymn J

(3.192)

[ J

with the generalized mass and stiffness matrices given by (3.184). 3.3.8 Variational Models In general, exact solutions for the dynamic response of laminated plates are not available and variational approximation methods can be used. According to the first-order shear deformation plate (FSDT) theory, the strain energy in a laminated plate is given by (3.90). The constitutive equations (3.99) and (3.103) can be written in matrix form as

Q = Ay. With this notation, the strain energy in the plate can be written as

U = \ f [ejAeo + KTDK + 2CJBK] dQ + \ [ yTAydQ.

(3.194)

For a symmetric laminate, the B matrix is zero and the inplane and transverse motions are uncoupled. In addition, if the effects of shear deformation are neglected (classical plate theory), the last term in (3.194) can be neglected and the strain energy becomes KTDicd£2

U = 2

(3.195)

Jn

when only out-of-plane deformations are considered. Using (3.94), the kinetic energy for a symmetric plate subjected to transverse deformations can be written as

T= =

\ L {h{ij2°+/3^'+^

}dQ

(3 l96)

*

when the effect of rotatory inertia are neglected, h = 0, and only the first term is left in the integrand of (3.196). For plates subjected to a distributed pressure q in the transverse direction only, the potential energy of the external forces can be written as V = - f qwodQ.

(3.197)

76

3 Impact Dynamics

With the Rayleigh-Ritz variational approximation method, the transverse displacements are taken as N

where the approximation functions 0/ must satisfy the essential boundary conditions and where the c, are constants to be determined. Substituting (3.198) into (3.195)-(3.197) yields U = -cT 2

<S>friDi(x,y)=xm-lyn-i

(3.205a)

0,-Oc, y) = xmyn(x - a)(y - b)

(3.205b)

4>i(x,y) = xm+lyn(y-b)

(3.205c)

for FFFF, SSSS, and CSFS plates respectively. Abrate (1995e) study the free vibrations of rectangular plate with intermediate line supports. With r supports located along the lines x = a\, a2, • • •, &r and s supports along the lines y = b\, £2, • . . , b s the approximation functions were taken as

4>i(x, y) = xm+ayn+\x

r

s

j=\

k=i

- aYiy - b)8 JJ(JC - aj) JJ(y - bk).

(3.206)

Following the same approach, polynomial approximation can be developed for other geometries. For example, for triangular plates with one edge along the x-axis, the approximation functions can be taken as (Abrate 1996a) 0;(x, y) = xm-lyn+a(cy

- bxf [bx + (a - c)y - abf

(3.207)

where a, /3, and y account for the support conditions along the sides v = 0, cy — bx — 0, and bx + (a — c)y — a = 0 and are taken to be -1,0, 1 for free, simply supported, and clamped edges, respectively. Example 3.10: Free Vibration of Plate with Intermediate Line Supports Consider a graphite-epoxy square plate with simple supports along the four edges and line supports along the lines x = a/4 and y = a/2, where a is the length of theside. The elastic properties ofthe material are E\ = 181.0 GPa, E2 = 10.30 GPa, V12 = 0.28, Gn = 7.17 GPa. The natural frequencies are nondimensionalized as follows: Q2 = co2pha4/(DnD22)l/2. Thefirstsix natural frequencies for angle-ply laminates are given in Table 3.4 as a function of the fiber orientation. The approximation functions are taken as &(*, y) = xay?(x - a)(y -

78

3 Impact

Dynamics

Table 3.4. Natural frequencies of graphite-epoxy angle-ply, two-way-two-span square plates Fiber orientation (degrees)

0 15 30 45 60 75 90

Natural frequencies (rad/s)

57.52 63.74 70.80 75.09 81.64 86.16 85.17

63.00 70.53 81.41 92.65 110.4 116.5 101.5

103.3 123.3 158.3 147.0 135.3 127.1 130.5

124.2 145.7 161.4 162.0 159.4 152.3 132.1

168.6 170.6 170.5 198.8 202.4 160.8 142.9

171.4 175.4 188.7 237.5 224.4 186.8 154.4

Table 3.5. Natural frequencies of clamped, elliptical, isotropic plate

1 9x9 Lam* 2 9x9 Lam 3 9x9 Lam 4 9x9 Lam 5 9x9 Singh**

10.2158 10.2160 27.3774 27.4773 56.8004 56.8995 97.5989 97.5984 149.6378 149.66

21.2604 21.2601 39.4974 39.4976 71.5912 71.5902 115.6089 115.6084 171.0975 171.10

21.2604 21.2601 55.9758 55.9773 90.2352 90.2380 137.2739 137.2686 196.2046 198.55

34.8772 34.8786 69.8580 69.8557 113.2753 113.2661 164.3236 164.3248 229.8105 229.81

34.8770 34.8786 77.0367 77.0443 140.7441 140.7461 195.3101 195.3398 266.2457

39.771 39.7712 88.0479 88.0472 150.0907 150.0889 255.1315 255.0946 350.4704

*Lametal. (1992). **Singh and Chakraverty (1994). The first six natural frequencies have converged for the first four significant figures when an 8 x 8 approximation is used. That is, a and f$ vary from 1 to 8, and TV = 64 in the displacement approximation (3.198). Example 3.11: Free Vibration of Elliptical Plate For clamped, isotropic, elliptical plates, the approximation functions are taken as ;, the boundary conditions (3.208) yield four equations that must be satisfied simultaneously: 1 ( - k\ • SS - CC)

-k\ ( - k'2 • CC - SS)

-1 ( - l\ • SH + CH)

-k\ ( - JkJ • CH + SH)

k[ r

. (k 2 • CC - SS)

r

( - k 2 - SS - CC)

r

(k 2 • CH + SH)

(kr2 • SH + C H ) .

(3.209)

80

3 Impact Dynamics Table 3.6. Natural frequencies (rad/s) of aluminum beam

Mode (1) 1 2 3 4 5 6

Experimental (2)

Cantilevered beam (3)

H&J* (4)

Elastically supported (5)

122.7 766.86 2131.6 4157.8 6818.64 10019.1

148.912 933.203 2612.93 5120.11 8463.48 12642.2

131.5 790.1 2148 4176 6868 10065

122.683 797.393 2240.33 4294.40 6818.64 9890.68

*Hassiotis and Jeong (1995). where

k\ =

k[ =

k>2-

k r2

(3.210)

and SS = :

3/L),

CC = cos(ftL),

SH = sinh(#L),

CH = cosh(#L). (3.211) For nontrivial solutions, the determinant of the matrix of the coefficients must vanish. For a given set of spring constants, the natural frequencies and mode shapes can be determined by finding the zeroes of a 4 x 4 determinant. The support stiffnesses are selected to minimize some objective measure of the difference between predicted and measured values of a set of natural frequencies: (3.212) 1=1

where £2; is the measured natural frequency, i is the predicted value, and N is the number of modes considered. Example 3.12: Identification of Boundary Conditions for an Aluminum Beam In this example, a 25.4-mm-wide, 6.35-mm-thick, 495.3-mm-long aluminum beam of uniform cross section is assumed to be clamped at one end and free at the other. The modulus of elasticity and the density of the material are E = 11 MPa and p = 2210 kg/m3, respectively. The natural frequencies predicted using classical cantilever boundary conditions (Table 3.6, column 3) are significantly higher that the experimental values (column 2). At x = 0, the support provides

81

33 Plate Theories Table 3.7. Natural frequencies (rad/s) of composite plate

Mode (1) 1 2 3 4 5

Experimental (2)

Finite element (3)

Cantilever beam (4)

Elastically supported

399.3 1113 2507.3 3992.1 7012.0

453.6 — 2826.4 4193.2 7859.6

453.254 — 2840.50 — 7953.47

399.300 — 2527.58 — 7011.96

(5)

some flexibility, and the best values for the rotational and translational spring constants are found to be k[ = 732,560 N/m, k\ = 668 N • m/rad. Example 3.13: Identification of Boundary Conditions for a Composite Plate Proper modeling of the support conditions for composite plates subjected to impact loading has long been recognized as a problem needing attention. Exjperiments were conducted on 3-layer graphite-epoxy specimens with a ply thickness of 0.015 in. and a total thickness of 0.045 in. The width was 2 in., the length 6 in., and the measured material properties are E\ = 19.832 Msi, E2 = 1.603 Msi, v\2 = 0.314, Gu = 0.926 Msi, p = 0.058 lb/in.3. Specimens were clamped at one end, and the natural frequencies and mode shapes were determined experimentally. Free vibrations were studied using a finite element model with an 8 x 17 mesh of 4 noded isoparametric plate elements, assuming the specimen to be clamped along the edge x = 0. The predicted natural frequencies (Table 3.7, column 3) are significantly higher than those measured (column 2). Since the material properties are known accurately, the discrepancy is expected to come from imperfect boundary conditions. Experiments and finite element results indicate that, for this example, modes 1,3, and 5 are pure bending modes and modes 2 and 4 involve torsional motion. Results obtained using the Bernoulli-Euler beam theory with cantilever boundary conditions (column 4) show that the bending modes are predicted accurately and that shear deformation effects are small because the specimens are thin. The difference between the finite element results (column 3) and the cantilever beam results (column 4) is due to the effect of shear deformation. Using the present approach, the support at the root is modeled by two linear springs whose stiffnesses were determined by minimizing the error measure EB for the first three bending modes. Using k[ = 3595 lb/in. and k\ = 684.0 lb • in./rad, excellent agreement is obtained between experimental results in column 2 and the predicted frequencies in column 5.

82

3 Impact Dynamics 3.3.10 Summary

In this section, the derivation of three plate theories were reviewed: the classical plate theory, the first-order shear deformation theory, and a higher-order plate theory. One static example illustrated the fact that as the ratio between the length of the side and the thickness of the plate becomes small, shear deformation effects become significant. Loading a plate with a concentrated force creates a singularity at the point of application of that force, which results in slow convergence in the solution procedure. In practice, loads are introduced through a small patch, and under such a loading, convergence problems are avoided and realistic distributions of transverse shear forces are obtained. Harmonic wave propagation analysis confirms the effect of shear deformation and indicates that the effects of rotary inertia are small in the range in which the plate theory is applicable. The bending-twisting coupling terms have a significant effect with four-ply laminates but are negligible when there are eight plies or more. Since there are only a few cases of plates for which closed-form solutions can be found, a variational approximation method capable of handling many complex cases was presented. Actual boundary conditions are often different than the ideal conditions and will significantly affect the dynamics of the structure. A procedure to determine the actual boundary conditions has been presented. 3.3.11 Exercise Problems 3.6

3.7 3.8

3.9

3.10

Use a one-term polynomial approximation in the Rayleigh-Ritz method to determine the fundamental natural frequency of a rectangular, simply supported plate. Compare the results with the exact solution given by (3.182). Using the classical plate theory, derive an exact solution for the deflection of a simply supported plate subjected to uniformly distributed static load. Using the first-order shear deformable plate theory, derive an exact solution for the deflection of a simply supported rectangular plate subjected to uniformly distributed static load. Assume that the laminate layup is specially orthotropic. Investigate the effect of shear deformation as a function of the ratio between the length of the side of the plate and the thickness. Derive a one-term Rayleigh-Ritz approximation for the fundamental natural frequency of an orthotropic rectangular plates with all four edges fully clamped. Use a polynomial approximation function. Develop an exact solution for the deflection of a rectangular, simply supported plate subjected to a force applied in its center. Assume that

3.4 Impact Models

3.11

83

force is applied as (1) a concentrated force and (2) a uniform pressure applied on a small square patch centered at the center of the plate. Plot the displacements along one line of symmetry of the plate, and investigate the effect of patch size and the number of terms retained in the solution. Develop a solution for the dynamic response of a rectangular, simply supported plate subjected to step load applied in its center. Compare this solution with the solution given by Medick (Section 3.3.7) for the transient response of an infinite plate to the same load. Show that the solution for an infinite plate is valid for very short times. That is when the disturbance has not yet reached the boundary and reflected back.

3.4 Impact Models Several types of mathematical models are used to study the impact of a structure by a foreign object. In certain cases, the contact force history can be accurately determined by modeling the structure by an equivalent spring-mass system. When the structure behaves quasi-statically, it is also possible to calculate the maximum contact force by assuming that when the contact force reaches its maximum, the sum of the strain energy in the structure and the energy required for indentation is equal to the initial kinetic energy of the projectile. This energybalance approach is useful when one is interested not in the complete contact force history but rather only in maximum contact force. When the dynamics of the structure must be more accurately accounted for, more sophisticated models are needed. In this section, the various models used for impact analysis are discussed, and examples are presented to illustrate various features of the impact event.

3.4.1 Spring-Mass Models Spring-mass models are simple and provide accurate solutions for some types of impacts often encountered during tests on small-size specimens. The most complete model (Fig. 3.15) consists of one spring representing the linear stiffness of the structure (Kbs), another spring for the nonlinear membrane stiffness, a mass M2 representing the effective mass of the structure, the nonlinear contact stiffness, and Mi, the mass of the projectile. From the free body diagrams of the two masses Mi and M2, we obtain the equations of motion: rjci + P = o, mx2 + Kbsx2 + Kmx$ - P = 0.

(3.213)

84

3 Impact Dynamics

E

T' x2

T

Figure 3.15. Spring-mass model. P is the contact force which, as discussed in Chapter 2, is a highly nonlinear function of the indentation x\ — JC2, which can be expressed as P = P(Xl-x2)

(3.214)

when x\ > x2. When x\ < *2, contact ceases, P = 0, and (3.208) govern the free vibration of the model. The dynamics of the system described by (3.208) and (3.209) and the initial conditions *i(0) = V,

*i (0) = * 2 (0) = 0

(3.215)

can be studied numerically. When geometrical nonlinearities and the indentation are negligible, the model can be significantly simplified to a single degree of freedom system with the equation of motion M'x + Kbsx = 0.

(3.216)

In that model, the effective mass of the structure is neglected and the structure and the projectile move together as soon as contact is made (JCI = x2 = x). The general solution to (3.216) is x = A sin cot + B cos cot

(3.217)

where to1 = Kbs/M\. The constants A and B are determined from the initial conditions (3.215), which give the result V x = —sincot. CO

(3.218)

3.4 Impact Models

85

Since the contact force P is equal to the force in the linear spring Kbs, the contact force history is given by F = Kbsx = V(KbsMi)i

sincot

(3.219)

for cot < n. When cot > n (3.214) predicts a negative contact force, which is impossible because contact between the projectile and the structure is unilateral. Therefore, separation occurs for t = Tc = TT/CO. The contact duration Tc increases with the mass of the projectile and decreases as the stiffness of the structure increases: Tc = n(Mx/Kbs)l

(3.220)

Equation (3.219) shows that the maximum contact force is directly proportional to the impact velocity and also increases with both the square root of the stiffness of the structure and the square root of the mass of the projectile. The maximum contact force is often plotted versus the initial kinetic energy of the projectile. For a given projectile (3.219) predicts that the maximum contact force increases with the square root of the kinetic energy. Example 3.14: Impact on a Half-Space Consider the impact on a half-space made out of steel by a 10-mm-radius steel ball with an initial velocity of 10 mm/s. The mass of the impactor is 32.24 g, Young's modulus is taken as 215.8 GPa, the density as 7966 kg/m3, and the contact stiffness as 1.538 x 1010 N/m 3/2 . In this case, there is no overall deflection of the target, so the motion of the projectile is governed by (3.213), where x\ represents both the displacement of the projectile and the indentation of the half-space and P = kcxx . This nonlinear equation of motion was solved using Newmark's step-by-step integration method with a time step of 2 /xs. The contact force history is given by the solid line in Fig. 3.16. The contact duration is 170 /xs, and the maximum contact force is 6.96 N. Some investigators linearize the contact law in order to avoid numerically solving a nonlinear differential equation. In this case, taking P = Ka, the equation of motion of the projectile is given by (3.216), the contact force is given by (3.219), and the contact duration is given by (3.220), where Kbs is replaced by K. If K is determined from (3.219) so that the maximum contact force matches that determined numerically (K = 1.503 x 107 N/m), the contact duration is significantly underestimated (Fig. 3.16). If K is determined from (3.220) so that the contact duration matches the numerically determined contact duration (K = 1.101x107 N/m), the maximum contact force is severely underestimated (Fig. 3.16). Therefore, for impacts dominated by local indentation, the use of linearized contact laws leads to significant errors.

3 Impact Dynamics

86 87-

\

/ /

/ / / .*

6-

^^ ^^

5-

\

\

\

••••»

\ \ \*. \ ^* •\

/ /

90.

'/ 7/

4-

x x

'' • /

•' -7

o

LL 3 -

\

/ .7 ///

2-

/

'•' i K f

0

\ \

#. 1 - //

I 0 - !/ /

V

i

i

50

100

\

\ V• \ \\ 150

Time (/JS) Figure 3.16. Impact of a sphere on a half-space.

3.4.2 Energy-Balance Models Another approach for analyzing the impact dynamics is to consider the balance of energy in the system. The initial kinetic energy of the projectile is used to deform the structure during impact. Assuming that the structure behaves quasistatically, when the structure reaches its maximum deflection, the velocity of the projectile becomes zero and all the initial kinetic energy has been used to deform the structure. The overall deformation of the structure usually involves bending, shear deformation, and for large deformations, membrane stiffening effects. Local deformations in the contact zone also are to be considered. For impacts that induce only small amounts of damage, the energy needed to create damage can be neglected. Therefore, the energy-balance equation can be written as

where the subscripts b, s, and m refer to the bending, shear, and membrane components of the overall structural deformation, and Ec is the energy stored in the contact region during indentation. It is always possible to express the

3.4 Impact Models

87

force-deflection relation in the form P = KbsW + KmW3

(3.222)

where Kbs is the linear stiffness including bending and transverse shear deformation effects, Km is the membrane stiffness, and W is the deflection at the impact point. Then Eb + Es + Em= l-Kbs Wlm +X-Km

Our partners will collect data and use cookies for ad personalization and measurement. Learn how we and our ad partner Google, collect and use data. Agree & close